# electronic and transport properties of nanotubes

Embed Size (px)

TRANSCRIPT

Jean-Christophe Charlier*

Unité de Physico-Chimie et de Physique des Matériaux (PCPM), Université Catholique de Louvain, 1 Place Croix du Sud, B-1348 Louvain-la-Neuve, Belgium

Xavier Blase†

Université de Louvain, F-69000, France, Laboratoire de Physique de la Matière Condensée et Nanostructures, Université Lyon I, CNRS, UMR 5586, Domaine scientifique de la Doua, F-69622 Villeurbanne Cedex, France

Stephan Roche‡

Commissariat à l’Energie Atomique, DSM/DRFMC/SPSMS/GT, 17 rue des Martyrs, 38054 Grenoble Cedex 9, France

!Published 16 May 2007"

This article reviews the electronic and transport properties of carbon nanotubes. The focus is mainly theoretical, but when appropriate the relation with experimental results is mentioned. While simple band-folding arguments will be invoked to rationalize how the metallic or semiconducting character of nanotubes is inferred from their topological structure, more sophisticated tight-binding and ab initio treatments will be introduced to discuss more subtle physical effects, such as those induced by curvature, tube-tube interactions, or topological defects. The same approach will be followed for transport properties. The fundamental aspects of conduction regimes and transport length scales will be presented using simple models of disorder, with the derivation of a few analytic results concerning specific situations of short- and long-range static perturbations. Further, the latest developments in semiempirical or ab initio simulations aimed at exploring the effect of realistic static scatterers !chemical impurities, adsorbed molecules, etc." or inelastic electron-phonon interactions will be emphasized. Finally, specific issues, going beyond the noninteracting electron model, will be addressed, including excitonic effects in optical experiments, the Coulomb-blockade regime, and the Luttinger liquid, charge density waves, or superconducting transition.

DOI: 10.1103/RevModPhys.79.677 PACS number!s": 73.63.Fg, 73.22.!f, 78.67.Ch, 61.46.Fg

CONTENTS

I. Introduction 678 II. Structure of Carbon Nanotubes 679

III. Electronic Properties of Carbon Nanotubes 681 A. From graphite to nanotubes 682 B. Tight-binding model of graphene 683 C. Zone-folding approximation 684

1. Metallic nanotubes 684 2. Semiconducting nanotubes 684

D. Band structures and densities of states 686 E. Band structures in a magnetic field 688

1. Aharonov-Bohm quantum phase 688 2. Parallel field: The band-gap opening and

orbital degeneracy splitting 689 3. Perpendicular field: The onset of Landau

levels 691 F. Curvature effects: Beyond the zone-folding model 692 G. Nanotube bundle and multiwall system 694 H. Structural defects in carbon nanotubes 695

1. Finite length and capping topologies 695 2. Connecting nanotubes 696 3. Vacancies, adatoms, Stone-Wales, etc. 697

I. Optical properties and excitonic effects 698 IV. Transport Properties of Carbon Nanotubes 700

A. Preliminary remarks 700 B. The clean limit 702

1. Ballistic motion and conductance quantization 702

2. Transport properties of CNT-based junctions and contact resistance 702

C. Effect of disorder on transport 704 1. Electronic eigenstates and pseudospin

symmetry 704 2. Long-range disorder and the absence of

backscattering 705 3. Short-range disorder and elastic mean free

path: Model analysis 706 4. Influence of doping on transport properties 707 5. Multishell conduction 709

a. Commensurate multiwalled nanotubes 709 b. Incommensurate multiwalled nanotubes 710 c. Crossed carbon nanotubes junctions,

bending and twisting deformations 711 D. Quantum interference effects 711

1. Weak localization and the Aharonov-Bohm

*Electronic address: [email protected] †Electronic address: xbla[email protected] ‡Electronic address: [email protected]

REVIEWS OF MODERN PHYSICS, VOLUME 79, APRIL–JUNE 2007

0034-6861/2007/79!2"/677!56" ©2007 The American Physical Society677

nanotubes 712 2. From weak to strong localization 714

E. Inelastic scattering 714 1. Electron-phonon coupling 714 2. Inelastic transport length scales 716 3. Electron-electron scattering and

Luttinger-liquid models 717 4. Transport spectroscopy in the Coulomb

blockade regime 721 F. Superconducting and charge-density-wave

instabilities 722 G. Field emission from nanotubes 724

V. Conclusion 726 Acknowledgments 726 References 726

I. INTRODUCTION

The physics of one-dimensional !1D" systems has been a rich and active playground for theorists for more than 50 years, with major conceptual breakthroughs arising from the specific properties of the confined electron gas. While the reduced dimensionality is often used in intro- ductory textbooks as a convenient way to simplify the analytic study of electronic properties, the enhanced in- teraction between electrons in 1D yields several insta- bilities that are not reproduced by standard tools devel- oped for 3D solids. This richness and complexity involved in extending the basics of condensed matter physics to low-dimensionality systems explain the wealth of work and theories developed to deal with 1D solids or molecular chains.

The difficulty in synthesizing clean 1D systems with metallic behavior has for many decades confined this theoretical work to formal developments and unverified predictions. However, progress in synthesis and charac- terization techniques in the late 1970s allowed a con- frontation between theory and experiments. Besides these fundamental aspects, the technological interest in controlling the properties of nanosized and/or plastic conductors was a strong driver for exploring this field. The attribution of the chemistry Nobel prize in 2000 to A. J. Heeger, A. G. MacDiarmid, and H. Shirakawa for the “discovery and development of conductive poly- mers” was a clear recognition from the community of the importance, and the difficulty, of obtaining conju- gated one-dimensional metallic systems. Further, even when metallic, the conductivity in such systems has been shown to usually remain very low, with in most cases polaron-assisted transport leading to very large effective masses for the carriers. As a paradigmatic example, the conducting !and even superconducting" properties of DNA, at the frontiers of physics, chemistry, and biology, are currently generating fierce controversies in the lit- erature.

The field of nanotubes has strongly benefited from this broad fundamental and technological interest. Not only can nanotubes be metallic, they are also mechani-

cally very stable and strong, and their carrier mobility is equivalent to that of good metals, suggesting that they would make ideal interconnects in nanosized devices. Further, the intrinsic semiconducting character of other tubes, as controlled by their topology, allows us to build logic devices at the nanometer scale, as already demon- strated in many laboratories. Finally, the large fullerene community !yet another area recognized by the Nobel prize in chemistry in 1996", and the even larger family of researchers interested in carbon-based systems, natu- rally joined this novel and promising field. This merging of interests and communities can certainly explain the formidable success and burgeoning activity generated by the discovery of nanotubes in 1991.

A nanotube is a honeycomb lattice rolled into a hol- low cylinder with nanometric diameter and "m length. Depending on the community, specific interests, and tar- geted applications, nanotubes are regarded as either single molecules or quasi-one-dimensional crystals with translational periodicity along the tube axis. As there are an infinite number of ways of rolling a sheet into a cylinder, the large variety of possible helical geometries, defining the tube chirality, provides a family of nano- tubes with different diameters and microscopic struc- tures. Some properties of these nanotubes, such as the elastic ones, can be explained within a macroscopic model of a homogeneous cylinder. Others depend cru- cially on the atomic configuration. For instance, the elec- tronic and transport properties, which constitute the scope of the present review, are certainly among the most significant physical properties of carbon nanotubes, and crucially depend on the diameter and chirality. This dependence on the atomic configuration, an effect ex- plained below, is quite unique in solid-state physics. This sensitivity constitutes a challenge for synthesis tech- niques, since well-controlled properties are often de- sired, but it is also a source of innovation for applica- tions.

In the following sections, we show how carbon nano- tubes can be either !semi"metallic or semiconducting, with a band gap varying from zero to a few tenths of an eV, depending on their diameter and chirality. Further, the band gap of semiconducting tubes, or the energy difference between the peaks in the electronic density of states !the so-called van Hove singularities", can be shown to first order to be simply related to the tube diameter. Such remarkable results can be obtained from a variety of considerations, starting from the so-called band-folding approach, based on knowledge of the elec- tronic properties of the graphene sheet, to the direct study of nanotubes using semiempirical tight-binding ap- proaches. The comparison with more sophisticated ab initio calculations, and with available experimental re- sults, allows us to set the limits of these simple treat- ments, with the introduction of finer considerations, such as curvature or trigonal warping effects.

Knowledge of the electronic properties of nanotubes further permits one to study their response to external probes. This is a crucial issue as it conditions most of the potentiality for the integration of tubes in real devices

678 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

and allows us to relate the structural and electronic properties with the experimental optical, Raman, etc., spectra. In particular, the effect of a magnetic field on the electronic band structure, the optical absorption and emission spectra, and finally the transport properties of tubes will be presented.

The tremendous importance of the transport proper- ties of nanotubes, from both a fundamental and techno- logical point of view, justifies devoting the second part of this review to that subject. First, the main characteristics of ballistic transport will be clarified, followed by a few analytical results about the absence of backscattering in the presence of long-range disorder and the derivation of the elastic mean free path induced by short-range dis- order. All transport regimes will be reviewed in the pres- ence of elastic disorder, starting with the simple Ander- son model, followed by an extended analysis of more realistic disorders such as chemical substitutions or func- tionalization, topological defects, and so on. Quantum interference effects will then be addressed with a focus on weak- and strong-localization regimes, in light of re- cent experiments. Further, the contribution of inelastic scattering mechanisms !through electron-electron and electron-phonon interactions" will be scrutinized, with a discussion of the inelastic scattering times and decoher- ence mechanisms. As a specific case of transport !or tun- neling", with much technological importance, the physics of field emission from nanotubes will be briefly pre- sented.

Several topics strongly related to quantum confine- ment and dimensionality effects will be addressed at the end of this review. At the heart of the complex behavior of 1D systems, the physics of the Luttinger-liquid transi- tion will be highlighted and the signature of this transi- tion in available transport experiments will be put in perspective. Coulomb-blockade effects and their mani- festation in transport measurements will then be sum- marized. Finally, the competing charge-density-wave !or Peierls" and superconducting instabilities upon switching on the electron-phonon interaction, observed experi- mentally, will be discussed.

The contents of the present review are theoretical, and experimental results are used primarily to provide the necessary and crucial evidence for validation of the theory. As a matter of fact, the difficulty in performing the synthesis and characterization of well-defined and isolated nanotubes has on many occasions granted to theory the important, but also dangerous, role of predic- tion. In return, these experimental difficulties have fos- tered the elaboration of original and creative experi- mental techniques. As emphasized below, most of the theoretical predictions seem now to be confirmed by many experimental results.

Even with a focus on theoretical results, space limita- tions impose a drastic, and necessarily subjective, selec- tion of topics and references. Thorough lists of refer- ences and a more complete picture !with, e.g., a description of the synthesis and characterization tech- niques" can be found in the excellent books devoted to the subject !Dresselhaus et al., 1996, 2001; Endo et al.,

1996; Ebbesen, 1997; Saito et al., 1998; Harris, 1999; Tománek and Enbody, 1999; Reich et al., 2004; Loiseau et al., 2006".

II. STRUCTURE OF CARBON NANOTUBES

Carbon nanotubes were discovered and first charac- terized in 1991 by Iijima from NEC laboratories !Japan" !Iijima, 1991". This discovery was made possible thanks to the use of state-of-the-art transmission microscopy. The first nanotubes discovered were made of several concentric cylindrical-like shells regularly spaced by an amount of about 3.4 Å as in conventional graphite materials !Fig. 1, left". These multiwall nanotubes !MWNTs" were first synthesized with diameters ranging from a few nanometers to several hundred nanometers for the inner and outer shells, respectively. As for the length, MWNTs extending over several microns are cur- rently synthesized.

Shortly after the discovery of multiwall carbon nano- tubes, single-wall carbon nanotubes !SWNTs" were syn- thesized in abundance using arc-discharge methods with transition-metal catalysts !Bethune et al., 1993; Iijima and Ichihashi, 1993". A carbon nanotube made of a single graphite layer !the graphene sheet" rolled up into a hollow cylinder is called a single-wall nanotube. These tubes have quite small and uniform diameter, on the or- der of 1 nm=10!9 m. This unprecedentedly small diam- eter, combined with the crystalline perfection of the atomic network, explains why these objects were quickly considered as the ultimate carbon-based 1D systems.

Crystalline ropes !or bundles" of SWNTs, with each rope containing tens to hundreds of tubes of similar di- ameter, closely packed in a hexagonal configuration, have also been synthesized using a laser vaporization method !Guo et al., 1995" and arc-discharge and chemi- cal vapor deposition !CVD" techniques !Fig. 1, right". Various synthesis methods have provided ample amounts of sufficiently characterized samples for study- ing the fundamental properties of SWNTs.

Because the microscopic structure of SWNTs is closely related to that of graphene, the tubes are usually labeled in terms of the graphene lattice vectors. As illus- trated in Fig. 2 a single-wall carbon nanotube is geo- metrically obtained by rolling up a single graphene strip !Saito et al., 1998". Its structure can be specified or in- dexed by its circumferential vector !Ch", as defined by the chiral vector !AA! in Fig. 2" which connects two crystallographically equivalent sites !A and A!" on a graphene sheet. In this way, a SWNT’s geometry is com- pletely specified by a pair of integers !n ,m" denoting the relative position Ch=na1+ma2 of the pair of atoms on a graphene strip which, when rolled onto each other, form a tube !a1 and a2 are unit vectors of the hexagonal hon- eycomb lattice; see Fig. 2".

This chiral vector Ch defines the circumference of the tube. The diameter dt of the nanotube can thus be esti- mated from

679Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

dt = #Ch#/# = a #

$n2 + nm + m2, !1"

where a is the lattice constant of the honeycomb net- work: a=$3$acc !acc%1.42 Å, the C-C bond length". The chiral vector Ch uniquely defines a particular !n ,m" tube, as well as its chiral angle %, which is the angle between Ch and a1 !zigzag direction of the graphene sheet; see Fig. 2". The chiral angle % can be calculated as follows:

cos % = Ch · a1

2$n2 + nm + m2 . !2"

The value of % is in the range 0& #%#&30°, because of the hexagonal symmetry of the graphene lattice. This chiral angle % also denotes the tilt angle of the hexagons with respect to the direction of the nanotube axis. Nanotubes of the type !n ,0" !%=0° " are called zigzag tubes, because they exhibit a zigzag pattern along the circumference. Such tubes display carbon-carbon bonds parallel to the nanotube axis. Nanotubes of the type !n ,n" !%=30° " are called armchair tubes, because they exhibit an armchair pattern along the circumference. Such tubes display carbon-carbon bonds perpendicular to the nanotube axis. Both zigzag and armchair nanotubes are achiral tubes, in contrast with general !n ,m#n#0" chiral tubes !Fig. 3".

The geometry of the graphene lattice and the chiral vector determine not only the diameter of the tube, but also the unit cell and its number of carbon atoms. The smallest graphene lattice vector T perpendicular to Ch

FIG. 1. High-resolution transmission electron microscopy pictures of a multiwall carbon nanotube !left" and a bundle of single- wall nanotubes !right", illustrating two different possible geometries for nanotubes. Courtesy of Gavillet, 2001.

FIG. 2. Graphene honeycomb network with lattice vectors a1 and a2. The chiral vector Ch=5a1+3a2 represents a possible wrapping of the two-dimensional graphene sheet into a tubular form. The direction perpendicular to Ch is the tube axis. The chiral angle % is defined by the Ch vector and the a1 zigzag direction of the graphene lattice. In the present example, a !5,3" nanotube is under construction and the resulting tube is illustrated on the right.

FIG. 3. Atomic structures of !12,0" zigzag, !6,6" armchair, and !6,4" chiral nanotubes.

680 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

defines the translational period t along the tube axis. The lattice vector T can also be expressed in terms of the basis vectors a1 and a2 as T= t1a1+ t2a2. Using Ch ·T =0, the expressions for t1 and t2 are given by

t1 = 2m + n

, !3"

where NR is the greatest common divisor of !2m+n" and !2n+m". The length of the translational vector t is given by

t = #T# = $3a$n2 + nm + m2/NR. !4"

The nanotube unit cell is thus formed by a cylindrical surface with height t and diameter dt. The number of carbon atoms per unit cell NC can also be expressed as a function of n and m:

NC = 4!n2 + nm + m2"/NR. !5"

The symmetry of carbon nanotubes can be described by the so-called line groups, which are full space groups of one-dimensional systems including translations in addi- tion to the point-group symmetries like rotations or re- flections. The carbon-nanotube line groups are nonsym- morphic groups as they always contain a screw axis. Every !n ,m" carbon nanotube belongs to a different line group !Damnjanovic et al., 1999; Reich et al., 2004". Only

armchair !n ,n" and zigzag !n ,0" tubes with the same n belong to the same symmetry group. Moreover, by start- ing with a single carbon atom and successively applying all symmetry operations of the line group, the whole tube is constructed. However, for many applications, such as optical transitions or first-order Raman scatter- ing, it is not necessary to work with the full line group, the point group being quite sufficient. These point groups are Dq for chiral nanotubes !n ,m#n#0" and D2nh for achiral tubes such as !n ,n" or !n ,0". After the symmetry operations of the nanotube have been deter- mined using its point group and its most basic structural properties !diameter, chirality, lattice, and reciprocal lat- tice vectors, as summarized in Table I", the correspond- ing graphene strip can be constructed and rolled up into a cylinder. The next step is now to predict its electronic behavior.

III. ELECTRONIC PROPERTIES OF CARBON NANOTUBES

Carbon nanotubes are characterized by two types of bond, in analogy with graphene, which exhibits so-called planar sp2 hybridization. Among the four valence orbit- als of the carbon atom !the 2s, 2px, 2py, and 2pz orbitals, z perpendicular to the sheet", the !s ,px ,py" orbitals com- bine to form in-plane ' !bonding or occupied" and '*

TABLE I. Structural parameters for a !n ,m" carbon nanotube. In this table, n, m, t1, t2 are integers.

Symbol Name Formula Value

a lattice constant a=$3acc%2.46 Å acc%1.42 Å

a1, a2 basis vectors !$3 2

; 1 2 "a, !$3

$3 ;1"2#

a , ! 1

$3 ;!1"2#

a

Ch chiral vector Ch=na1+ma2&!n ,m" !0& #m#&n"

dt tube diameter dt=

2n+m

T translational vector T= t1a1+ t2a2&!t1 , t2" gcd!t1 , t2"=1a

t1= 2m+n

NC number of C atoms per unit cell NC=

4!n2+nm+m2" NR

agcd!n ,m" denotes the greatest common divisor of the two integers n and m.

681Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

!antibonding or unoccupied" orbitals !Fig. 4". Such orbit- als are even with respect to planar symmetry. The ' bonds are strong covalent bonds responsible for most of the binding energy and elastic properties of the graphene sheet. The remaining pz orbital, pointing out of the graphene sheet, is odd with respect to the planar symmetry and cannot couple with the ' states. The lat- eral interaction with neighboring pz orbitals !labeled the pp# interaction" creates delocalized # !bonding" and #*

!antibonding" orbitals. In analogy, the ' bonds in the nanotube form a hexagonal network which strongly con- nects the carbon atoms in the cylinder wall of the tube. The # bonds are perpendicular to the surface of the nanotube and are responsible for the weak interaction between SWNTs in a bundle, similar to the weak inter- action between carbon layers in pure graphite !Charlier et al., 1991". The energy levels associated with the in- plane ' bonds are known to be far away from the Fermi energy in graphite !Fig. 4, right" and thus do not play a key role in its electronic properties. In contrast, the bonding and antibonding # bands cross the Fermi level

at high-symmetry points in the Brillouin zone of graphene !Wallace, 1947". For a good understanding of the electronic properties of SWNTs, the electronic struc- ture of graphene will be briefly discussed in the next section.

A. From graphite to nanotubes

Although graphite has been studied for decades, graphene was only isolated experimentally in 2004 after a long struggle !Novoselov et al., 2004". Further, and de- spite early predictions !Wallace, 1947", its remarkable conducting properties, in which electrons mimic the be- havior of massless, relativistic particles, have only been observed recently !Novoselov et al., 2005; Zhang et al., 2005".

The electronic bands of graphene along the high- symmetry M-(-K directions are presented in Fig. 5. The # and #* bands cross at the vertices of the hexagonal Brillouin zone !Fig. 6". Such vertices are labeled by their momentum vector usually written as K. Consequently, graphene is a special semimetal whose Fermi surface is reduced to the six distinct K points of the hexagonal Brillouin zone. Close to the Fermi energy, the # and #*

bands are nearly linear, in contrast with the quadratic energy-momentum relation obeyed by electrons at band edges in conventional semiconductors. This linear energy-momentum relation of electrons will explain the extremely good conductivity in graphene and bears much importance in the Luttinger-liquid !LL" behavior for low-energy excitations in nanotubes !see Sec. IV.E.3".

The bonding and antibonding ' bands are well sepa- rated in energy !)10 eV at (". These bands are fre- quently neglected in semiempirical calculations as they are too far away from the Fermi level to play a role in the electronic properties of graphene. The remaining two # bands can be simply described with a rather simple tight-binding Hamiltonian, leading to analytical solutions for their energy dispersion and the related eigenstates. This simple approach can be further ex-

FIG. 5. Electronic properties of graphene. !a" Electronic band structure of graphene. The bonding ' and antibonding '* bands are separated by a large energy gap. The bonding # !last valence" band and antibonding #* !first conduction" band cross at the K points of the Brillouin zone. The Fermi energy is set to zero, and * indicates the work function. Above the vaccuum level !dotted horizontal line", the states of the continuum are difficult to describe and merge with the '* bands. !b",!d" # state at K and !c",!e" ' state at (, seen from above and from the side of the graphene plane. Note that the # wave function cancels on a hexagonal sublattice due to the exp!iK ·r" phase factor. The # !'" state is odd !even" with respect to the graphene plane reflection. Courtesy of Fernández-Serra, 2006.

FIG. 4. The ' bonds in the carbon hexagonal network connect the carbon atoms and are responsible for the binding energy and the elastic properties of the graphene sheet !left". The # bonds are perpendicular to the surface of the sheet. The cor- responding bonding and antibonding ' bands are separated by a large energy gap !right", while the bonding and antibonding # states lie in the vicinity of the Fermi level !EF". Adapted from Loiseau et al., 2006.

682 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

tended to study the properties of nanotubes by combin- ing these analytic results with the requirement that the wave functions in tubes must satisfy the proper bound- ary conditions around the tube circumference. This is what we show in the next sections.

B. Tight-binding model of graphene

As mentioned in the previous section, the graphene plane is a hexagonal lattice with two atoms per unit cell !A and B" and a basis defined by vectors !a1 ,a2" !see Fig. 6". The condition ai ·bj=2#+ij allows one to obtain the reciprocal-lattice vectors !b1 ,b2". Every carbon atom possesses four valence electrons !two 2s and two 2p elec- trons". When the atoms are placed onto the graphene hexagonal lattice, as in Fig. 6, the electronic wave func- tions from different atoms overlap. However, such an overlap between the pz orbitals and the s or px and py electrons is strictly zero by symmetry. Consequently, the pz electrons, which form the # bonds in graphene, can be treated independently of other valence electrons. Within this #-band approximation, the A atom !B atom" is uniquely defined by one orbital per atom site pz!r !rA" 'pz!r!rB"(.

To derive the electronic spectrum of the total Hamil- tonian, the corresponding Schrödinger equation has to be solved, and by applying the Bloch theorem, the wave functions can be written as follows:

,!k,r" = cA!k"pz A!k,r" + cB!k"pz

eik·!pz!r ! rB ! !" , !8"

where k is the electron momentum !the quantum num- ber", Ncells is the number of unit cells in the graphene sheet, and ! is the cell position index. The spectrum is derived by solving the Schrödinger equation which re- duces to a 2$2 matrix diagonalization:

*HAA ! E HAB

HAA!k" = 1

A,!!- , !10"

HAB!k" = 1

B,!!- , !11"

with the notation pz A/B,-=pz!r!rA/B!-". Here we have

neglected the overlap matrix elements S= ,pz A # pz

B- be- tween neighboring pz orbitals !neglect of overlap inte- grals defines the so-called orthogonal tight-binding schemes". After simple manipulations and restricting in- teractions to first nearest neighbors only, one gets

HAB!k" = ,pz A,0#H#pz

B,0- + e!ik·a1,pz A,0#H#pz

B,!a1-

B,!a2- = ! .0/!k" , !12"

with .0 the transfer integral between first-neighbor # orbitals !a typical value for .0 is 2.9 eV", /!k"= !1 +e!ik·a1 +e!ik·a2", and ,pz

A,0#H#pz A,0-= ,pz

B,0#H#pz B,0-=0 as

the energy reference. The dispersion relations are then readily obtained:

E±!k" = ± .0$3 + 2 cos!k · a1" + 2 cos!k · a2" + 2 cos'k · !a2 ! a1"( , !13"

which can be further developed as

E±!kx,ky" = ± .0$1 + 4 cos $3kxa

2 cos

kya 2

!14"

by setting a=$3acc !acc=1.42 Å". The k= !kx ,ky" vectors that belong to the first hexagonal Brillouin zone !BZ"

constitute an ensemble of available electronic momenta. In Fig. 7, these simple tight-binding dispersion relations are represented with dashed lines along high symmetry directions of the BZ, defined by the ( and M points together with the six BZ vertices !K points".

With one pz electron per atom in the #-#* model !the three other s, px, and py electrons fill the low-lying ' band", the !!" band !negative energy branch" in Eq. !14"

FIG. 6. Brillouin zone and reciprocal space. !a" Basis vectors in the hexagonal lattice of graphene. !b" Brillouin zone. The corresponding reciprocal basis vectors read b1=b!1/2 ,$3/2" and b2=b!1/2 ,!$3/2", with b=4# /a$3.

683Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

is fully occupied, while the !0" branch is empty. These occupied and unoccupied bands cross at the K points 'one verifies that /!k=K"=0(. The Fermi level EF !or charge-neutrality point" is therefore the zero-energy ref- erence in Fig. 7, and the Fermi surface is defined by the set of K points. Since the occupied and unoccupied bands do cross, the graphene sheet displays a metallic !zero-gap" character. However, as the Fermi surface is of zero dimension !since it is reduced to a discrete and fi- nite set of points", the term semimetal is usually used.

This simple orthogonal tight-binding model yields # and #* zone-center ( energies which are symmetric !±.0" with respect to EF. In fact, the antibonding !unoc- cupied" #* bands are located at a higher energy if the overlap integral S is not set to zero !see Fig. 7". A better, but more complicated, #-#* parametrization can be found in Reich, Maultzsch, Thomsen, and Ordejón !2002" where a careful comparison between ab initio and various tight-binding schemes is presented for graphene and several nanotubes. The main advantage of the present nearest-neighbor approximation is the very simple analytical expression for the # electronic states of graphene.

C. Zone-folding approximation

Due to periodic boundary conditions along the cir- cumferential direction of the tube, the allowed wave vectors “around” the nanotube circumference are quan- tized: they can take only a set of discrete values. In con- trast, the wave vectors along the nanotube axis remain continuous !for infinite tubes". Plotting these allowed vectors for a given nanotube onto the Brillouin zone of graphene generates a series of parallel lines. The length, number, and orientation of these cutting lines depend on the chiral indices !n ,m" of the nanotube. The basic idea behind the zone-folding approximation is that the elec-

tronic band structure of a specific nanotube is given by superposition of the graphene electronic energy bands along the corresponding allowed k lines. This is what we explain now.

A specific carbon nanotube defines a unique chiral vector Ch= !n ,m" expressed in the basis !a1 ,a2" !Fig. 2" that fixes its symmetry and its diameter. As mentioned in Sec. II, the chiral vector length #Ch# equals $3acc$n2+nm+m2 or #dt !dt being the nanotube diam- eter". The application of periodic boundary conditions around the tube circumference leads to some restrictions on the allowed wave function quantum phase:

,k!r + Ch" = eik·Ch,k!r" = ,k!r" , !15"

with the vectors r and k taken on the tube surface. The first equality stems from the Bloch theorem. Depending on the tube symmetry, that is, on the chiral vector Ch = !n ,m", two situations can occur.

1. Metallic nanotubes

We make an analysis in the neighborhood of the Fermi surface, so that we write k=K++k, with +k small, taking, e.g., K= !b1!b2" /3= !0,4# /3a", so that k = !+kx ,4# /3a++ky". When eiK·Ch =1 !which is possible only when n!m=3l, with l an integer", then the con- straint on the wave function becomes +k ·Ch=2#q !q in- teger". Each index q defines a line of allowed k vectors, and each line contributes to one occupied # band and one unoccupied #* band. The condition n!m=3l is al- ways satisfied for armchair tubes and for the subset of the !n ,0" zigzag tubes with n multiples of 3. Rewriting the dispersion relation in the general case as E2!kx ,ky" =.0

2#/#2 and performing a second-order perturbation ex- pansion in the vicinity of the K points, one finally ob- tains #/!kx ,ky"#2% 3

4 !+kx 2++ky

2"+O!+k3" !with +kx and +ky related by +k ·Ch=2#q". Close to EF, the dispersion re- lation then reads E±!+k"% ± !$3a /2".0.+k., a linear energy-momentum relation mentioned above. There- fore, states arbitrarily close in energy to the Fermi level can be found for q=0 and the system is metallic !see Fig. 8". The Fermi velocity vF=$3a.0 /21= 3

2acc.0 /1 is typi- cally given by vF%8$105 m s!1 for .0=2.9 eV. The lin- ear band dispersion close to EF will be shown to have useful consequences.

A simple expression for the eigenstates can also be derived close to EF within the same type of approxima- tion. Such an expression will be used in Sec. IV.C.2 to show that elastic backscattering is quenched in nano- tubes if the disorder is long ranged. One notes that, for a general helical symmetry, the full properties of the eigenstates can be derived by constructing generalized Bloch states satisfying helical !rototranslation" symme- tries !Mintmire et al., 1992".

2. Semiconducting nanotubes

The second possible choice for !n ,m" nanotubes is given by the condition n!m=3l±1. In this situation

FIG. 7. Limitations of the #-#* model. !a" Ab initio !solid lines" and nearest-neighbor orthogonal tight-binding 'dashed lines, from Eq. !14"( # and #* electronic bands for graphene. !b" Difference 2E between the ab initio and tight-binding band structures. Adapted from Reich, Maultzsch, Thomsen, and Or- dejón, 2002.

684 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

eiK·Ch = ±e2i#/3, and one gets +k= !2# / #Ch#"!q±1/3"3!

+k.3. with 3! and 3. the basis vectors along the Ch and T directions, respectively, where T is the translational vector along the tube axis, as defined in Sec. II. By fol- lowing a similar calculation as for the prior case, one obtains in the vicinity of the Fermi level a new disper- sion relation, namely,

Eq ±!k." % ±

+ k. 2, !16"

where the integer variable q counts the available bands, whereas k. is the part of the wave vector that continu- ously describes the states within a given subband !and associated with the direction parallel to the tube axis".

This case leads to an obvious gap opening at the Fermi level !Fig. 9" since

Eq=0 + !k. = 0" ! Eq=0

! !k. = 0" = 2#a.0

1. !17"

It appears that 2Eg 1 decreases as the inverse of the tube

diameter dt !dt= #Ch# /#". For a very large diameter, one finds as expected a zero-gap semiconductor since we re- cover the graphene sheet. For realistic tubes, with, e.g., a diameter of 1.4 nm 'helical vector !17,0"(, one gets 2Eg

1

%0.59 eV. This 1 /d dependence of the gap on the diam- eter relies on the assumption of a linear dispersion of the bands around EF, a result first derived by White and Mintmire !1998". In reality, the bands are not linear away from EF, an effect called trigonal warping !Saito, Dresselhaus, and Dresselhaus, 2000" which induces a de- pendence of the band gap not only on the diameter, but on the !n ,m" indices as well.

In relation to the study of transport properties an im- portant quantity linked to the dispersion relation is the so-called effective mass of the charge carriers. In semi- conducting nanotubes, this quantity can be derived from Eq. !16",

Eq=0 ± = ± $!m*vF

2"2 + !1k.vF"2,

defining m*=2#1 /3#Ch#vF, which is thus inversely pro- portional to the nanotube diameter and tends to zero as the diameter tends to infinity !graphene limit". This con- cept has been used !Zhou et al., 2005" to estimate the charge mobility properties in semiconducting nanotubes.

In summary, early theoretical calculations !Hamada et al., 1992; Mintmire et al., 1992; Saito et al., 1992" showed that the electronic properties of carbon nanotubes are very sensitive to their geometric structure. Although graphene is a semimetal, theory has predicted that car- bon nanotubes can be metals or semiconductors with an energy gap that depends on the tube diameter and he- licity, i.e., on the indices !n ,m". These results can be simply understood within a band-folding picture, as il- lustrated in the present section. This approach is made relatively simple in nanotubes because of the special shape of the graphene Fermi surface and the restriction of the electronic bands to the #-#* manifold.

FIG. 8. The band-folding scheme. !a" Brillouin zone of graphene. The white rectangle is the Brillouin zone associated with the four-atom cell with lattice vectors Ch /n=a1+a2 and T !T=a1!a2 for an armchair tube". Thick lines are the allowed k lines for the !5,5" armchair tube. To obtain the !5,5" band struc- ture in the band-folding approach, fold the colored corners onto the rectangular cell and superimpose the graphene energy bands calculated along the obtained thick lines of length 2# / #T#. In particular, the K points are folded at two-thirds of (X !or its inversion symmetry image". The bands are indexed by the integer q such that k ·Ch=2#q. In the corresponding !5,5" tube, q is also the azimuthal quantum number. !b" Disper- sion relations E±!kx ,ky" for the graphene plane, together with that of an armchair nanotube !bold line".

FIG. 9. Dispersion relations E±!kx ,ky" for the graphene plane, together with that of a zigzag semiconducting nanotube !bold line".

685Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

When forming a tube, owing to the periodic boundary conditions imposed in the circumferential direction, only a certain set of k vectors in the graphene BZ are al- lowed. This allowed set of Bloch momenta depends on the diameter and helicity of the tube. Whenever the al- lowed k vectors include the point K, the system is a metal with a nonzero density of states at the Fermi level, resulting in a one-dimensional metal with two bands dis- persing linearly close to EF. When the K point is not included, the system is a semiconductor with a small band gap that depends mainly on the diameter. In this case, the conduction- and valence-band edges come from states with k vectors located on the allowed line!s" closest to the K point.

Within the zone-folding approximation, the general rules for the metallicity of single-wall carbon nanotubes are as follows: a nanotube defined by the !n ,m" indices will be metallic !semiconductor" if n!m=3l, with l an integer !n!m=3l±1". Consequently, most carbon nano- tubes are semiconductors and only a fraction !1/3" are metallic !or semimetallic".

To conclude this subsection, we note that the index q, as defined above by the condition k ·Ch=2#q 'Eq. !15"( is also the azimuthal quantum number associated with the states on the corresponding allowed k line. This quantum number therefore characterizes the behavior of eigenstates with respect to rotations around the axis that transform the tube into itself. It can be used in par- ticular to study, on the basis of symmetry-related selec- tion rules !Vucovic et al., 2002", the effect of a perturba- tion on various subbands and their mixing upon static !e.g., tube squashing, interaction with a substrate, etc." or time-dependent !e.g., optical excitation" perturba- tions.

D. Band structures and densities of states

As the nanotubes are one dimensional, their Brillouin zone is one dimensional as well, with zone edges usually labeled X, namely, X= ± !# /T"!., with !. and T defined above. The nanotube band structure is therefore repre- sented along the (X direction !(X! with X!=!X sym- metric by time reversal". In the band-folding approach, one obtains therefore a superposition of all allowed Eq

±!k." graphene eigenvalues, with q the allowed line in- dex !two bands per line" and k. the continuous momen- tum along 3. !from now on, as there is only one direc- tion, we drop the . subscript and write k. =k". One says that the allowed k lines are “folded” onto the (X direc- tion 'see Fig. 8!a" for armchair tubes(. We now study the band structure and related density of states of !n ,m" tubes as given by the band folding of the #-#* bands of graphene within the orthogonal tight-binding scheme presented above.

The electronic band structure of an armchair !5,5" car- bon nanotube is presented in Fig. 10. Six bands for the conduction and an equal number for the valence states are observable. However, four of them are degenerate, leading to ten electronic levels in each case, consistent

with the ten hexagons around the circumference of the !5,5" nanotube. Indeed, the bands coming from two al- lowed lines with opposite q index, for q= ±1 to q= ±4 'see Fig. 8!a"(, are degenerate by symmetry. For all arm- chair nanotubes, the energy bands exhibit a large degen- eracy at the zone boundary, where k= ±# /a !X point", so that Eq. !14" becomes E!k= ±# /a"= ±.0. This comes from the absence of dispersion along the segments con- necting the neighboring centers of the BZ sides !the M points", an effect that will yield the so-called trigonal warping of the bands as discussed below. The valence and conduction bands for armchair nanotubes cross at k=kF= ±2# / !3a", a point that is located at two-thirds of (X 'Fig. 8!a"(. This means that the original K vertices of the original graphene hexagonal BZ are folded at two- thirds of the (X line !or its inversion symmetry image". As discussed above, the !5,5" armchair nanotube is thus a zero-gap semiconductor which will exhibit metallic conduction at finite temperatures, since only infinitesi- mal excitations are needed to promote carriers into the conduction bands.

The density of states !DOS" 2N /2E represents the number of available states 2N for a given energy inter- val 2E !2E!0". This DOS is a quantity that can be measured experimentally under some approximations. The shape of the density of states is known to depend dramatically on dimensionality. In 1D, as shown below, the density of states diverges as the inverse of the square root of the energy !1/$E" close to band extrema. These “spikes” in the DOS are called Van Hove singularities !VHSs" and manifest the confinement properties in di- rections perpendicular to the tube axis. As carbon nano- tubes are one dimensional, their corresponding DOSs exhibit such a spiky behavior at energies close to band edges !see Fig. 10". The position of these Van Hove sin- gularities can be analytically derived from the dispersion relations. The density of states is defined by

FIG. 10. Band structure and density of states for a !5, 5" arm- chair nanotube within the zone-folding model. The 1D energy dispersion relations are presented in the '!3.0 ;3.0( energy in- terval in dimensionless units !.0 being the nearest-neighbor C-C tight-binding overlap energy /2.9 eV". The energy bands are plotted along the X-(-X direction. The Fermi level is lo- cated at zero energy.

686 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

4!E" = 1 5

Tr'+!E ! H"( , !18"

where +!E!H" is the spectral measure; the trace is ex- panded within a complete basis, and 5 is the volume of the considered system. For the set of eigenvalues Eq

s !k", where s=± refers to the sign of the solution in Eq. !14", the DOS can be expressed as

4!E" = 2 5

= 2 5

$k 1!1

, !19"

where kqs are the roots of the equation E!Eq s !k"=0,

while 5=4##Ch# /$3a2 is the volume !surface" of the re- ciprocal space for each allowed state divided by the dis- tance between allowed lines in the graphene Brillouin zone !see above". In the vicinity of K, where one can use the linear energy-momentum relation, the contribution of k to the density of states is related to

1 $Eq s !k"

2 , !20"

where 6qs gives the energy position of the Van Hove singularities. In the vicinity of EF, those positions are given by #6qs#=$3.0a2k!

q /2 with 2k! q = 2!k!K" ·Ch / #Ch#2

=2##3q!n+m# /3#Ch#. Hence #6qs#=#.0acc#3q!n +m# / #Ch#, and one finally obtains the density of states

4!E" = 2a

2 . !21"

For all metallic nanotubes, the density of states per unit length along the nanotube axis is a constant at the Fermi energy !EF" and can be expressed analytically !Mintmire and White, 1998":

4!6F" = 2$3acc/!#.0#Ch#" . !22"

Beyond the linear-band approximation, one can rewrite Eq. !14" for metallic armchair !n ,n" nanotubes to obtain the following band dispersion relation:

Eq ±!k" = ± .0$1 + 4 cos

ka 2

, !23"

where q=1,2n corresponds to the discrete part of the wave vector !band index" and k is the continuous part of the wave vector, describing states in a specific band !!#7ka7#". The positions of the Van Hove singulari- ties can then be derived analytically directly from Eq. !23", and a simple calculation gives 6q,s=±= ±.0 sin q# /n. In Fig. 10, the spikes in the DOS are localized at 6q=1,10;s=±= ±.0 sin q# /5.

We now turn to zigzag tubes. The calculated 1D dis- persion relations E!k" for the !9,0" and !10,0" zigzag nanotubes are illustrated in Figs. 11 and 12, respectively. As expected, the !9,0" tube is metallic, with the Fermi surface located at (, whereas the !10,0" nanotube exhib-

its a finite energy gap at (. In particular, in the case of the !10,0" nanotube, there is a dispersionless energy band at E /.0= ±1, which gives a singularity in the DOS at these particular energies. For a general !n ,0" zigzag nanotube, when n is a multiple of 3, the energy gap at k=0 !( point" becomes zero. However, when n is not a multiple of 3, an energy gap opens at (. The correspond- ing densities of states have a zero value at the Fermi energy for the semiconducting nanotube and a small nonzero value for the metallic one.

It should be noted that the k values for the band crossing at EF in metallic nanotubes are k= ±2# /3T or k=0 for armchair or zigzag tubes, respectively. These k values are also the locations of the band gaps for semi- conducting zigzag nanotubes. The same k values denote as well the positions of the energy gaps !including zero energy gaps" for the general case of chiral nanotubes. In Fig. 13, the dispersion relations E!k" for the !8,2" chiral nanotube are shown. Since n!m is a multiple of 3, this nanotube exhibits a metallic behavior with a band cross- ing at k= ±2# /3T. Other chiral nanotubes, like the !9,6", display a zero energy gap at k=0. The DOS of chiral

FIG. 11. Band structure and density of states for a !9, 0" zigzag nanotube within the zone-folding model. The Fermi level is located at zero energy.

FIG. 12. Band structure and density of states for a !10,0" zigzag nanotube within the zone-folding model. The Fermi level is located at zero energy.

687Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

nanotubes !see Fig. 13" also displays Van Hove singulari- ties as for achiral tubes !Charlier and Lambin, 1998; Mintmire and White, 1998; White and Mintmire, 1998".

In semiconducting zigzag or chiral nanotubes, the band gap 'as expressed by Eq. !17"( is independent of the chiral angle and varies inversely with the nanotube diameter: 2Eg

1=2.0acc /dt !in the linear-band approxima- tion". Density-of-states measurements by scanning tun- neling spectroscopy !STS" provide a powerful tool for probing the electronic structure of carbon nanotubes. It can be shown, indeed, that under some assumptions the voltage-current derivative dI /dV is proportional to the DOS. These experiments !Odom et al., 1998; Wildöer et al., 1998" confirmed that the energy band gap of semi- conducting tubes is roughly proportional to 1/dt and that about 1/3 of nanotubes are conducting, while the other 2/3 are semiconducting. Resonances in the DOS have also been observed experimentally !Odom et al., 1998; Wildöer et al., 1998" on both metallic and semicon- ducting nanotubes whose diameters and chiral angles were determined using a scanning tunneling microscope !STM" !Venema et al., 2000". Several other experimental techniques, such as resonant Raman scattering !Jorio et al., 2001" and optical absorption and emission measure- ments !Bachilo et al., 2002; O’Connell et al., 2002; Le- febvre et al., 2003", have also confirmed this structure in Van Hove singularities of the electronic densities of states in single-wall carbon nanotubes.

E. Band structures in a magnetic field

The application of a uniform external magnetic field has profound consequences on the electronic band struc- ture of carbon nanotubes. There exist two cases of high symmetry for the direction of the magnetic field with respect to the nanotube axis. When the magnetic field is applied parallel to the tube axis, electrons within the nanotube are influenced by the electromagnetic poten- tial, whose dominating effect is to add a new phase fac- tor to the quantum wave function !with subsequent modification of the associated momentum", and in the

cylinder geometry this phase factor will be driven in a periodic fashion by the magnetic flux threading the nanotube cross section. This quantum phenomenon was first described theoretically by Aharonov and Bohm !1959", whereas field-periodic oscillations of the magne- toresistance were experimentally measured in ordinary metallic rings !Webb et al., 1985", opening a new field for mesoscopic physics !Imry, 1997".

Given that the metallic or semiconducting character of carbon nanotubes results from the existence of the allowed momentum k at the K points of the hexagonal Brillouin zone, the superimposed Aharonov-Bohm phase factor, modulated by the field, will induce some field-dependent disruption of the initial eigenstate distri- bution in reciprocal space, with a first spectacular effect of the band gap opening for an initially metallic system, as first described by Ajiki and Ando !1993". In this sec- tion, we provide the basics for understanding the Aharonov-Bohm phenomenon in carbon nanotubes and its consequences on the electronic spectrum. In Sec. IV.D.1, its corresponding effects on transport properties will be further described.

1. Aharonov-Bohm quantum phase

To further deepen and illustrate these effects, let us describe the modifications of the quantum phase factor, driven by the vector potential A and associated with the external magnetic field B=B!ux ,uy ,uz" !with B=rotA". Within the tight-binding scheme, the Bloch functions in the static B can be written as

,!k,r" = 1

$N ) R

eik·Rei8R9!rR" .

With R a lattice vector and 8R the phase factor associ- ated with the magnetic field, it can be shown that 8R!r" =3R

r A!r!"dr!=30 1!r!R" ·A!R+:'r!R("d: !Luttinger,

1951", so that the total matrix elements of H= !p /2m !eA"2+V!r", in the presence of B, are simply obtained through multiplication of those in the zero-field case by the phase factor !Saito et al., 1998". For a general de- scription of the B-dependent band-structure effects, one possibility is to adopt the Cartesian basis !ex ,ey ,ez" where ez and ex are, respectively, taken along and per- pendicular to the tube axis. In the Landau gauge A =B!0,uzx ,uxy", the Aharonov-Bohm phase acquired during an electronic motion between an orbital located at !xi ,yi ,zi" and another located at !xj ,yj ,zj" can be eas- ily derived:

8ij = 2# *0

2 5 , !24"

where *0 is the quantum flux. This result is applicable whatever the direction of B with respect to the tube axis and gives the axial configuration for !ux=0,uz=1" and the perpendicular configuration for !ux=1,uz=0". This further allows us to compute the remormalized field- dependent coupling overlap between # orbitals, .ij!B"

FIG. 13. Band structure and density of states for a !8,2" chiral nanotube within the zone-folding model. The Fermi level is located at zero energy.

688 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

=.0 exp'!2i# /*0"3ri

2. Parallel field: The band-gap opening and orbital degeneracy splitting

In the axial case, however, the use of another basis set makes understanding of the Aharonov-Bohm effect straightforward. Indeed, if one considers the two- dimensional Cartesian coordinates r= !x , y" in the basis defined by the directions !Ch ,T", then the vector poten- tial is recast as A= !* / #Ch# ,0" and the magnetic phase factor between two # orbitals located at ri= !xi , yi" and rj= !xj , yj" is simply written as 8i!8j= i*!xi! xj" / #Ch#. Ac- cordingly, the periodic boundary conditions on the quan- tum phase will be modified as

,k!r + #Ch#" = eik·Chexp*!2#/*0"0 r

r+Ch

A!r!"dr!+,k!r" ,

and since the additional magnetic phase factor thus re- duces to 2#* /*0, the change in the quantum momentum becomes

3! ! 3!!*" = 2# #Ch# *q ±

/

*0 + , !25"

with /=0 for metallic tubes, and /= ±1 for semiconduct- ing tubes. In Fig. 14 the effect of this change in momen- tum is illustrated in reciprocal space. From Eqs. !16" and !25", the field-dependent gap oscillation for an initially metallic tube is obtained,

2EB = Eq=0 + !k.,*/*0" ! Eq=0

! !k.,*/*0" = 32Eg 1*/*0,

if *&*0 /2, where 2Eg 1=2#acc.0 /$3#Ch# denotes the gap

at zero flux as given by Eq. !17". If *0 /2&*&*0, then 2EB=32Eg

1#1!* /*0#, so that the band gap exhibits an

oscillation between 0 and 2Eg 1 with a period *0 !Ajiki

and Ando, 1993, 1994, 1996; Tian and Datta, 1994; Lin et al., 1995; Lu, 1995". For instance, 2EB675 meV at 50 T for the !22,22" tube !diameter63 nm", while 2EB 640 meV at 60 T for the !10,10" tube !diameter =1.4 nm". In addition, to obtain a field equivalent to * =*0 in nanotubes with diameters of 1, 10, 20, and 40 nm, one typically needs magnetic fields of 5325, 53, 13, and 3 T, respectively.

In addition to such *0-periodic band-gap oscillations, the Aharonov-Bohm effect more generally affects the whole subband structure, as evidenced by Van Hove sin- gularity splitting and shifts !Jiang et al., 2000; Roche et al., 2000; Shyu et al., 2003". These effects result from the influence of the magnetic field on the orbital degeneracy. Indeed, the initial symmetry of the carbon nanotubes implies that each available energy level is initially four- fold degenerate !including spin and orbital degeneracy". The orbital degeneracy is attributed to the symmetry between clockwise !0" and counterclockwise !!" elec- tronic motions around the tube. In the presence of an external magnetic field, electrons in degenerate !0" and !!" eigenstates will acquire opposite orbital magnetic moments ±"orb, which will thus produce an upshift of the energy of !0" and a downshift of the energy of !!", resulting in lifting the orbital degeneracy !or Van Hove singularity splitting".

This mechanism is illustrated in the DOS plots for the !5,5" and !10,10" tubes in Figs. 15 and 16, respectively, which are both metallic nanotubes at zero magnetic field !Roche et al., 2000". The calculations have been per- formed using a simple tight-binding model in the #-orbital approximation, while nearest-neighbor hop- ping integrals have been renormalized in the presence of a magnetic field using Eq. !24".

FIG. 14. Representation of the first Brillouin zone of a graphene sheet together with allowed states for an armchair tube !dashed lines" at zero flux. Modifications of allowed states in the vicinity of k points, under the effect of a magnetic field applied parallel to the tube axis !circles give the equipotentials close to the Fermi energy".

FIG. 15. !Color online" Density of states of the !5,5" carbon nanotube for several magnetic flux values: * /*0=0 !a", * /*0 =0.1 !b", * /*0=0.2 !c", and * /*0=0.5 !d". This is a metallic tube at zero magnetic flux but a gap opens up once a finite flux is applied and increases with the flux.

689Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

As predicted theoretically, by applying a finite mag- netic flux * threading the tube, the band gap opens and increases linearly with *, to reach a maximum value at half the quantum flux !*0 /2". Further, the band gap is linearly reduced until it finally closes back when the field reaches one quantum flux. The labels !a"–!e" in Fig. 16 are the DOSs for the !10,10" tube at * /*0= !a" 0, !b" 0.125, !c" 0.25, !d" 0.375, and !e" 0.5. For * /*0=0.125 'trace !b"(, one notices that in the vicinity of the charge- neutrality point !i.e., 6=0", a new VHS appears, indicat- ing the gap opening. In !c", !d", and !e", the gap is seen to increase, reaching its maximum value at * /*0=0.5. The evolution of the VHS is then reversed and the gap closes again at * /*0=1. For VHSs at higher energies !e.g., those located at 6q=1", the oscillatory behavior is slightly more involved: at low fields a splitting is observed for each VHS, which is followed by crossing at higher flux, and finally all VHSs return to the original positions when * /*0=1 !see the inset of Fig. 16".

In the case of armchair !n ,n" metallic tubes, the mag- nitude of the field-dependent splitting of the qth VHS can be analytically ascertained:

2EB!6q,*/*0" = 2.04sin #

q*0 5 . !26"

Semiconducting tubes 'i.e., !n ,m" tubes with n!m =3l±1 !l being an integer"( are affected in a similar way, but the gap expression is slightly different. One finds 2EB=2Eg

1#1!3* /*0# if 0&*&*0 /2 and 2EB=2Eg 1#2

!3* /*0# when *0 /2&*&*0. Hence, the initial zero- field energy gap !2Eg

1" continuously decreases with in- creasing *, to reach zero at *=*0 /3. The gap further opens as * increases from *0 /3, reaching a local maxi-

mum !2Eg 1 /2" at *=*0 /2, before closing again at *

=2*0 /3, and finally recovering its original value 2Eg 1 at

*=*0. In Fig. 17, the DOS of a 3-nm-diameter semicon- ducting single-walled tube for various magnetic flux is illustrated. One notes that magnetic-field-induced lifting of the spin degeneracy brings some additional contribu- tion to the total electron magnetic moment !Zeeman ef- fect". This effect has been shown to yield an energy level displacement between spin up and spin down, linear with the magnetic flux, but inversely proportional to the squared radius of the tube !Jiang et al., 2000".

The Van Hove singularity splitting was recently ob- served by spectroscopic experiments !Zaric et al., 2004". In addition, several experimental studies of electronic transport spectroscopy at low temperature in the Cou- lomb blockade regime !Kanda et al., 2002; Coskun et al., 2004; Jarillo-Herrero et al., 2004; Minot et al., 2004" or in the Fabry-Perot regime !Cao et al., 2004; Jarillo-Herrero et al., 2005" have also provided compelling evidences of the Aharonov-Bohm effect. The experimental estima- tion of the orbital magnetic moment was found to be of the order of %0.7–1.5 meV/T !Minot et al., 2004; Jarillo-Herrero et al., 2005".

Magnetoresistance oscillations were also a subject of intense controversy in the early stage of carbon nano- tube studies, since the origin and value of the Aharonov- Bohm oscillation period were apparently of different na- tures. Indeed, while some studies of large-diameter multiwall carbon nanotubes !Bachtold et al., 1999" first revealed clear signatures of weak localization, with negative magnetoresistance and !*0 /2"-periodic Aharonov-Bohm oscillations driven by quantum inter- ferences !Altshuler and Aronov, 1985", other reports as- signed their magnetoresistance oscillations to field- modulated band structure effects, assuming a negligible contribution from interference effects !Fujiwara et al., 1999; Lee et al., 2000". The superimposed contributions to the Aharonov-Bohm oscillations from both band- structure and quantum interferences effects have been clearly disentangled recently !Stojetz et al., 2005" and will be discussed in Sec. IV.D.1.

FIG. 16. Density of states of the !10,10" metallic tube as a function of energy for several magnetic flux values !see text". Curves have been vertically offset for clarity. Inset: Evolution of one VHS with magnetic flux. Adapted from Roche et al., 2000.

FIG. 17. Density of states of the !21,23" tube at zero and finite flux. Top inset: Expanded plot of the DOS. Bottom inset: Evo- lution of the VHS splitting 2B as a function of magnetic field.

690 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

3. Perpendicular field: The onset of Landau levels

In the situation where the magnetic field is applied perpendicular to the tube axis, the modifications of the electronic spectrum are profoundly different. First the two-dimensional vector potential within the Landau gauge for the nanotube surface is now given by A = „0, !#Ch#B /2#"sin!2#x / #Ch#"…, keeping !x , y" as the co- ordinates along the circumferential and nanotube axis directions. For evident symmetry reasons, the net mag- netic flux threading the tube is now zero. The phase fac- tors can be computed using either this basis or the Car- tesian basis defined earlier. The energy dispersion can then be evaluated as a function of magnetic field inten- sity !Ajiki and Ando, 1993, 1996; Saito et al., 1994". In Fig. 18, the dispersion relation of the energy E /.0 is reported as a function of the dimensionless wave vector k.#T# /2# !Saito et al., 1994", for several values of the dimensionless inverse magnetic length ;= #Ch# /2#!m, where !m=$1 /eB is the magnetic length !first cyclotron orbit radius".

As seen in Fig. 18, as the intensity of the magnetic field is enhanced, the subband dispersion is reduced, with a particularly strong effect in the vicinity of the charge-neutrality point. This onset of a Landau-type subband can be further rationalized analytically. Indeed, by using the k ·p method, an expression for the eigen- states under magnetic field close to the K points can be derived analytically for metallic tubes !see Sec. IV.C.1

for the zero-field case". The k ·p equation at the charge- neutrality point !"k=0" in the presence of a perpendicu- lar magnetic field can be decoupled into two equations !Ando and Seri, 1997":

4! $

$x +

k !x" = 0, !27"

k !x" = 0, !28"

,A!x" = *1 0 +FA!x", ,B!x" = *0

1 +FB!x" ,

FA!x" = 1

#Ch# +5 ,

FB!x" = 1

#Ch# +5 ,

where I0!2;2" is a modified Bessel function of the first kind. Note that for sufficiently large magnetic field !; <1" these wave functions become strongly localized in the circumference direction; that is, ,A!x" is a wave function localized around x= ± #Ch# /2 at the bottom side of the cylinder, whereas ,B!x" is localized around the

FIG. 18. Energy dispersion relation of a !10,0" tube as a function of the dimensionless wave vector ==k.#T# /2# for several values of the dimensionless inverse magnetic length ;. !a" ;=0.0, !b" 1.0, !c" 2.0, and !d" 3.0. !e", !f", !g" The energy at k. =0 as a function of ;2 /NR 'NR is the highest common divisor of !2n+m ,n+2m"( for tubes !20,0", !20,20", and !9,9", respectively. Adapted from Saito, Dresselhaus, and Dresselhaus, 1994.

691Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

top side x=0. As a result, the boundary condition on the wave function becomes irrelevant and the resulting band structures, starting from an initially metallic or semicon- ducting nanotube, become identical !Ajiki and Ando, 1993". For a small +k around the K points, the low- energy properties are described by an effective Hamil- tonian, which can be determined by the two degenerate states ,A and ,B as

Heff = * 0 ! i.0+kI0 !1!2;2"

+ i.0+kI0 !1!2;2" 0

whose eigenvalues are Eq=0 ± = ±.0#+k# /I0!2;2", with a

group velocity given by v=.0 /1I0!2;2", while the density of states becomes 4!EF"/I0!2;2" /#.0/e;

2 /$4#;2!;

<1" !Ando and Seri, 1997". The DOS at the charge- neutrality point thus diverges exponentially with in- creasing magnetic field. This is shown in Fig. 19 for the !10,10" tube for several magnetic field strengths.

Given the diameter-dependent scaling property of the band structure, the larger the tube diameter, the smaller the required value of the magnetic field to fully develop such a Landau subband at the charge-neutrality point. This effect has also been investigated analytically using a supersymmetry framework !Lee and Novikov, 2003". The appearance of the so-called Hofstadter butterfly was further explored numerically for large diameter nanotubes !Nemec and Cuniberti, 2006". As already seen in the field-dependent band structures !Fig. 18", the whole DOS also progressively degrades as the Landau subbands start to emerge within the whole spectrum, al- though strong mixing between high-energy subbands re- mains !Fig. 19".

As soon as ;= #Ch# /2#!m>1 is satisfied, the electronic spectrum becomes fully dominated by Landau levels. One finds that for tubes with diameters of 1, 10, 20, and 40 nm, the condition ;=1 corresponds to magnetic field strengths of 2635, 26, 6.6, and 1.6 T, respectively.

In each case, !m?!e !or @c-e<1" has to be further satisfied for clear observation of Landau quantization, where !e is the mean free path, @c=eB /m is the cyclo- tron frequency, and -e is the scattering time !this condi- tion is easily met at such high magnetic fields in carbon nanotubes since !e can be as long as 1 "m". Some signa- ture of such Landau level formation was first reported by Kanda and co-workers !Kanda et al., 2002".

F. Curvature effects: Beyond the zone-folding model

In the preceding sections, a model for the electronic properties of SWNTs was based on the confinement of electrons around the tube circumference, a confinement shown to induce selection on allowed k! Bloch vector components. As a matter of fact, since the states se- lected in the band-folding scheme were those of the pla- nar graphene sheet, curvature effects are neglected. However, carbon nanotubes are not just stripes of graphene but small cylinders. Carbon atoms are placed on a cylindrical wall, a topology that induces several ef- fects different from those of a planar graphene sheet: !a" the C-C bonds perpendicular and parallel to the axis are slightly different, so that the a1 and a2 basis vectors now have different lengths; !b" these bond length changes, and the formation of an angle for the two pz orbitals located on bonds not strictly parallel to the axis, yield differences in the three hopping terms .0 between a car- bon atom and its three neighbors; and !c" the planar symmetry is broken so that the # and ' states can mix and form hybrid orbitals that exhibit partial sp2 and sp3

character. Such curvature effect is not taken into ac- count in the zone-folding model of graphene, where the # orbitals cannot mix with the ' states as they show different parity with respect to planar reflection. In the present section, the effect of finite curvature on the elec- tronic properties of single-wall nanotubes will be inves- tigated.

The effects labeled !a" and !b" modify the conditions that define the k point at which occupied and unoccu- pied bands do cross !a point we label kF" and shift this Fermi vector kF away from the Brillouin zone corners !K point" of the graphene sheet !Kane and Mele, 1997; Yang and Han, 2000". For armchair nanotubes, taking curvature into account shifts the Fermi wave vector along an allowed line of the graphene Brillouin zone. Consequently, for symmetry reasons, armchair tubes al- ways preserve their metallic character with finite curva- ture. However, for metallic nonarmchair nanotubes, kF moves away from the K point perpendicularly to the allowed k lines such that the allowed 1D subband !k ,q" no longer passes through kF, opening a very small band gap at EF !see Fig. 20".

In summary, when accounting for curvature effects, the only zero-band-gap tubes are the !n ,n" armchair nanotubes. The !n ,m" tubes with n!m=3l, where l is a nonzero integer, are tiny-gap semiconductors. Armchair tubes are sometimes labeled type-I metallic tubes, while the others are of type-II. All other nanotubes are

FIG. 19. Density of states of the !10,10" tube in a perpendicu- lar magnetic field for several field strengths. The field strengths are expressed in terms of the dimensionless parameter ; = #Ch# /2#!m, where !m=$1 /eB is the magnetic length.

692 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

intermediate-gap !a few tenths of an eV" semiconduc- tors. For the tiny-gap semiconducting nanotubes, the so- called secondary gap !due to the curvature" depends on the diameter and the chiral angle, and scales as 1/dt

2

!Kane and Mele, 1997". For the quasimetallic zigzag nanotubes !chiral angle=0", this secondary gap is given by

2Eg 2 =

3.0acc 2

4dt 2 !30"

and is so small that, for most practical purposes, all n !m=3l tubes can be considered as metallic at room tem- perature !see Fig. 20". Density-of-states measurements by scanning tunneling spectroscopy !Ouyang et al., 2001b" confirm the expected 1/dt

2 dependence for three zigzag nanotubes and show that armchair nanotubes re- main truly metallic. Consequently, the band-folding pic- ture, based on the tight-binding approach !Hamada et al., 1992; Mintmire et al., 1992; Saito et al., 1992", contin- ues to be valid for large diameter tubes.

We now discuss point !c". For small tubes, the curva- ture is so strong that some rehybridization among the ' and # states appears. In such a case, the zone-folding picture may fail completely and ab initio calculations should be performed to predict the electronic properties of small diameter nanotubes. As an example, the ab ini- tio band structure of the !6,0" tube is shown in Fig. 21. These first-principles pseudopotential local density func- tional !LDA" calculations !Blase, Benedict, Shirley, and Louie, 1994" indeed revealed that hybridization effects can occur in small radius nanotubes sufficiently strong to significantly alter their electronic structure. Strongly modified low-lying conduction band states are intro- duced into the band gap of insulating tubes because of

hybridization of the '* and #* states. As a result, the energy gaps of some small radius tubes are decreased by more than 50%. In the specific case of the !6,0" tube, which is predicted to be a semimetal in the band-folding scheme, a singly degenerate hybrid '*-#* state !see Fig. 21" is found to lie 0.83 eV !at (" below the doubly de- generate state that forms the top of the valence band in the zone-folding model. This band overlap makes the !6,0" tube a true metal within the LDA, with a density of states at the Fermi level equal to 0.07 state/eV atom. The '*-#* hybridization can be clearly observed by drawing the charge density associated with the states around the Fermi level. Such states are no longer anti- symmetric with respect to the tube wall, with a clear “charge spilling” out of the tube. For nanotubes with diameters greater than 1 nm, these rehybridization '-# effects are unimportant. Further, as discussed above, symmetry considerations suggest that armchair tubes are less affected by such rehybridization.

Ultrasmall radius single-wall carbon nanotubes !diam- eter of about 4 Å" have been produced by confining their synthesis inside inert AlPO4-5 zeolite channels !with inner diameter of about 7.3 Å" !Wang et al., 2000". The diameter of these tubes gives them many unusual properties such as superconductivity !Tang et al., 2001". Such a narrow distribution of diameters around 4 Å re- duces the potential carbon nanotube candidates to three: the !3,3", !4,2", and !5,0". The properties of these ultrasmall tubes have already been extensively investi- gated by ab initio simulations !Dubay et al., 2002; Liu and Chan, 2002; Machón et al., 2002; Cabria et al., 2003". In particular, it was shown that the !5,0" tube, expected to be semiconducting following the band-folding picture, is actually a metal with two bands !one doubly degener- ate" crossing the Fermi level !yielding two different kF".

FIG. 20. Magnitude of primary !Eg 1" and secondary !Eg

2" gaps in carbon nanotubes with radii less than 15 Å. The primary gap !2Eg

1" scales as 1/R !top panel". The secondary gap !2Eg 2

or cuvature-induced gap" scales as 1/R2. The dots at 2Eg 1

=2Eg 2=0 correspond to the armchair nanotubes which always

preserve their metallic character. Adapted from Kane and Mele, 1997.

FIG. 21. Ab initio electronic band structure and density of states of a !6,0" carbon nanotube, illustrating the strong hybrid- ization that occurs between # and ' states in a small-diameter tube. A new band '* appears and crosses the # states around the center of the Brillouin zone. The Fermi level is at zero energy. Adapted from Blase, Benedict, Shirley, and Louie, 1994.

693Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

This is a clear manifestation of curvature effects. We will come back to such small tubes when discussing the Peierls and superconducting instabilities in Sec. IV.F. The armchair !3,3" tube remains semimetallic, but with a #-#* band crossing at EF that is displaced off its ideal 2(X /3 position, confirming as described above that arm- chair tubes are much less sensitive to curvature effects.

G. Nanotube bundle and multiwall system

From the previous section, we can deduce that only a special achiral subset of these carbon structures !arm- chair nanotubes" exhibits a true metallic behavior. Such metallic character can be explained by the high symme- try of these !n ,n" tubes, namely, the n vertical planes and glide planes. Incorporating an armchair tube into a bundle, or inside another nanotube as in a multiwall sys- tem, could modify its intrinsic electronic properties as the symmetry is lowered.

Single-wall carbon nanotubes are grown by a laser- ablation, arc-discharge, or CVD method and always oc- cur in bundles of 10–100 nanotubes. These bundles usu- ally consist of nanotubes with different chirality and slightly different diameter. Even a “perfect” crystal made of identical tubes will alter the properties of the constituent CNTs through tube-tube interaction. Indeed, first-principles calculations reveal that broken symmetry of the !10,10" tube caused by interactions between tubes in a bundle induces a pseudogap of about 0.1 eV at the Fermi energy !Delaney et al., 1998". This pseudogap strongly modifies many of the fundamental electronic properties of the armchair tubes, with a specific signa- ture in the temperature dependence of the electrical conductivity and in the infrared absorption spectrum.

In the limit of an isolated !10,10" tube, the two bands crossing at EF belong to different irreducible represen- tations with respect to the tube symmetry planes, so that crossing is allowed. Upon breaking of this symmetry by tube-tube interaction in the hexagonal bundle symmetry, these bands can mix and start to repel at EF !Fig. 22". The presence and magnitude !which depends inversely on the nanotube radius" of this pseudogap have been observed experimentally using low-temperature scan-

ning tunneling spectroscopy !Ouyang et al., 2001b". In contrast, if !6,6" nanotubes are arranged in a hexagonal lattice which fully preserves the D6h symmetry of the hexagonal packing, the band gap due to these intertube interactions is not observed !Charlier et al., 1995". A small rotation of the !6,6" tubes in such an arrangement would break the D6h symmetry of the !6,6" bundle and would open up this expected gap at the Fermi energy !Reich, Thomsen, and Ordejón, 2002".

Another possibility to tailor the electronic properties of nanotubes can be observed in the multilayering effect. In fact, the weak interaction between the concentric shells in a multiwall nanotube may have important ef- fects on the electronic properties of the constituent iso- lated nanotubes !Lambin et al., 1994; Kwon and Tománek, 1998". Interwall coupling, which, as just men- tioned, opens a pseudogap in bundles of single-wall nanotubes !due to symmetry lowering", may periodically open and close four such pseudogaps near the Fermi energy in a metallic double-wall nanotube upon rotation of its inner shell with respect to the nanotube axis.

Figure 23 illustrates the intriguing interplay between geometry and electronic structure during the rotation of an inside !5,5" armchair nanotube in an outside !10,10" nanotube !both tubes sharing the same axis". The indi- vidual !5,5" and !10,10" tubes are both metallic and show the preferred graphitic interwall separation of 3.4 Å when nested. To determine the electronic properties of the double-wall nanotube, a tight-binding technique with parameters determined by ab initio calculations for simpler structures has been used !Lambin et al., 1994; Kwon and Tománek, 1998". Due to the relatively high symmetry of the coaxial system, consisting of a D10h !5,5" nanotube nested inside a D20h !10,10" nanotube, the de- pendence of the intertube interaction on the tube orien- tation shows a periodicity of 18°. In the absence of the intertube interaction, the band structure of each tube is characterized by two crossing linear bands near EF, one for left- and one for right-moving electrons. The band structure of a pair of decoupled !5,5" and !10,10" nano- tubes, a mere superposition of the individual band struc- tures, is shown in Fig. 23!a". Switching on the intertube interaction in the !5,5"@!10,10" double-wall tube re-

FIG. 22. Band crossing and band repulsion. !a" Schematic diagram of the crossing of the two linear bands for an isolated !n ,n" carbon nanotube. One band has #-bonding character and the other has #-antibonding !#*" character. EF is the Fermi energy and k is the wave vector. !b" Repulsion of the bands due to breaking of mirror symmetry. Adapted from Delaney et al., 1998.

694 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

moves the near degeneracy of the bands near EF as well 'see Figs. 23!b" and 23!c"(. In the most stable orienta- tion, the double-wall system is still characterized by the D10h symmetry of the inner tube. The four bands cross, with a very small change in the slope 'Fig. 23!b"(. While the same argument also applies to the least-stable con- figuration, a markedly different behavior is obtained at any other tube orientation that lowers the symmetry, giving rise to four band crossings 'Fig. 23!c"(. This trans- lates into four pseudogaps in the density of states near EF.

At the Fermi level, the density of states of double-wall nanotubes is thus affected by the mutual orientation of the two constituent nanotubes, since the positions of the four pseudogaps depend significantly on it. The opening and closing of pseudogaps during the libration motion of the double-wall tube is a unique property that cannot be observed in single-wall nanotube ropes !Kwon and Tománek, 1998".

Finally, self-consistent charge-density and potential profiles for double-wall nanotubes, considering various chiralities, have been determined !Miyamoto et al., 2001" and demonstrate that the inner tube modifies the charge density associated with states near EF, even outside the outer tube. A significant amount of charge, originating mainly from # electrons, is transferred into an interwall state, related to the interlayer state in graphite. In the limit of small tubes, the significant evolution of the CNT work function with respect to diameter shows as well that charge transfer may occur from one tube to another.

H. Structural defects in carbon nanotubes

In the previous sections, curvature effects and inter- tube and intershell interactions have been shown to sig- nificantly modify the electronic properties of carbon nanotubes from those obtained by a simple band folding of the graphene band structure. However, until now, each constituent nanotube was assumed to be perfect. In reality, the intrinsic honeycomb network of CNTs is probably not as perfect as usually assumed. Defects like pentagons, heptagons, vacancies, adatoms, or substitu-

tional impurities have been proposed theoretically and recently observed experimentally !Hashimoto et al., 2004; Fan et al., 2005". These defects are found to modify, at least locally, the electronic properties of the host nanotubes. Consequently, the introduction of de- fects in the carbon network is an interesting way to tai- lor its intrinsic properties, enabling new potential nano- devices and fostering innovative applications in nano- electronics !Gómez-Navarro et al., 2005". The cases of chemical doping and functionalization will be explored in Sec. IV.C.4 where their effect on conductance will be analyzed.

1. Finite length and capping topologies

We have dealt so far with the properties of infinitely long nanotubes. In reality, nanotubes have a finite length !up to a few microns", a property which has two main consequences: !a" the confinement of the electronic states along the tube length; and !b" the disruption of the atomic network at the two ends, also labeled tips or apexes, with specific reconstructions and local electronic properties.

A conducting nanotube cut to a finite length should display standing waves characteristic of a one- dimensional particle-in-a-box model. Indeed, when elec- trons are confined in a box, quantum mechanics tells us that electrons can have only discrete values of kinetic energy. The energy spacing of the eigenvalues depends directly on the dimensions of the box: 2E=h2 /2mL2, with L the length of the box. If this energy spacing is much higher than the thermal energy !2E<kBT", there are only completely occupied and completely empty lev- els and the system is an insulator. Further, the eigen- states are standing waves of the form sin!kz", with k =2#m /L and m an integer !the variable z is along the nanotube axis".

These standing waves have been studied theoretically by Rubio et al. !1999", and the highest occupied molecu- lar orbital !HOMO", lowest unoccupied molecular or- bital !LUMO", and “tip states” associated with a typical finite-length tube are illustrated in Fig. 24. Such station- ary states have also been observed experimentally by

FIG. 23. Band structures of the same double-wall tube for different relative orientations. Near-degenerate bands with no gap characterize the !5,5"@!10,10" double-wall nanotube without intertube interaction !a". In the presence of intertube interaction, depending on the mutual tube orientation, the !5,5"@!10,10" system may show a zero gap !b" in the most symmetric !point group symmetry D10h" or four pseudogaps !c" in a less symmetric and stable configuration !point group symmetry C5". Adapted from Kwon and Tománek, 1998.

695Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

means of STS !Venema et al., 1999; Lemay et al., 2001" which essentially sees the square of the wave functions close to the Fermi level 'dI!V ,x" /dV/#,F!x"#2(. The STS scans display several maxima repeated with a peri- odicity :F60.74 nm. Such an observation requires a higher energy resolution than the eigenstate separation !2E" and an electron coherence length larger than the tube length, which was satisfied for Ltube/30 nm and T=4 K.

We now turn to the properties of tube tips or apexes. Due to the finite length, interesting structural features occur near t

Unité de Physico-Chimie et de Physique des Matériaux (PCPM), Université Catholique de Louvain, 1 Place Croix du Sud, B-1348 Louvain-la-Neuve, Belgium

Xavier Blase†

Université de Louvain, F-69000, France, Laboratoire de Physique de la Matière Condensée et Nanostructures, Université Lyon I, CNRS, UMR 5586, Domaine scientifique de la Doua, F-69622 Villeurbanne Cedex, France

Stephan Roche‡

Commissariat à l’Energie Atomique, DSM/DRFMC/SPSMS/GT, 17 rue des Martyrs, 38054 Grenoble Cedex 9, France

!Published 16 May 2007"

This article reviews the electronic and transport properties of carbon nanotubes. The focus is mainly theoretical, but when appropriate the relation with experimental results is mentioned. While simple band-folding arguments will be invoked to rationalize how the metallic or semiconducting character of nanotubes is inferred from their topological structure, more sophisticated tight-binding and ab initio treatments will be introduced to discuss more subtle physical effects, such as those induced by curvature, tube-tube interactions, or topological defects. The same approach will be followed for transport properties. The fundamental aspects of conduction regimes and transport length scales will be presented using simple models of disorder, with the derivation of a few analytic results concerning specific situations of short- and long-range static perturbations. Further, the latest developments in semiempirical or ab initio simulations aimed at exploring the effect of realistic static scatterers !chemical impurities, adsorbed molecules, etc." or inelastic electron-phonon interactions will be emphasized. Finally, specific issues, going beyond the noninteracting electron model, will be addressed, including excitonic effects in optical experiments, the Coulomb-blockade regime, and the Luttinger liquid, charge density waves, or superconducting transition.

DOI: 10.1103/RevModPhys.79.677 PACS number!s": 73.63.Fg, 73.22.!f, 78.67.Ch, 61.46.Fg

CONTENTS

I. Introduction 678 II. Structure of Carbon Nanotubes 679

III. Electronic Properties of Carbon Nanotubes 681 A. From graphite to nanotubes 682 B. Tight-binding model of graphene 683 C. Zone-folding approximation 684

1. Metallic nanotubes 684 2. Semiconducting nanotubes 684

D. Band structures and densities of states 686 E. Band structures in a magnetic field 688

1. Aharonov-Bohm quantum phase 688 2. Parallel field: The band-gap opening and

orbital degeneracy splitting 689 3. Perpendicular field: The onset of Landau

levels 691 F. Curvature effects: Beyond the zone-folding model 692 G. Nanotube bundle and multiwall system 694 H. Structural defects in carbon nanotubes 695

1. Finite length and capping topologies 695 2. Connecting nanotubes 696 3. Vacancies, adatoms, Stone-Wales, etc. 697

I. Optical properties and excitonic effects 698 IV. Transport Properties of Carbon Nanotubes 700

A. Preliminary remarks 700 B. The clean limit 702

1. Ballistic motion and conductance quantization 702

2. Transport properties of CNT-based junctions and contact resistance 702

C. Effect of disorder on transport 704 1. Electronic eigenstates and pseudospin

symmetry 704 2. Long-range disorder and the absence of

backscattering 705 3. Short-range disorder and elastic mean free

path: Model analysis 706 4. Influence of doping on transport properties 707 5. Multishell conduction 709

a. Commensurate multiwalled nanotubes 709 b. Incommensurate multiwalled nanotubes 710 c. Crossed carbon nanotubes junctions,

bending and twisting deformations 711 D. Quantum interference effects 711

1. Weak localization and the Aharonov-Bohm

*Electronic address: [email protected] †Electronic address: xbla[email protected] ‡Electronic address: [email protected]

REVIEWS OF MODERN PHYSICS, VOLUME 79, APRIL–JUNE 2007

0034-6861/2007/79!2"/677!56" ©2007 The American Physical Society677

nanotubes 712 2. From weak to strong localization 714

E. Inelastic scattering 714 1. Electron-phonon coupling 714 2. Inelastic transport length scales 716 3. Electron-electron scattering and

Luttinger-liquid models 717 4. Transport spectroscopy in the Coulomb

blockade regime 721 F. Superconducting and charge-density-wave

instabilities 722 G. Field emission from nanotubes 724

V. Conclusion 726 Acknowledgments 726 References 726

I. INTRODUCTION

The physics of one-dimensional !1D" systems has been a rich and active playground for theorists for more than 50 years, with major conceptual breakthroughs arising from the specific properties of the confined electron gas. While the reduced dimensionality is often used in intro- ductory textbooks as a convenient way to simplify the analytic study of electronic properties, the enhanced in- teraction between electrons in 1D yields several insta- bilities that are not reproduced by standard tools devel- oped for 3D solids. This richness and complexity involved in extending the basics of condensed matter physics to low-dimensionality systems explain the wealth of work and theories developed to deal with 1D solids or molecular chains.

The difficulty in synthesizing clean 1D systems with metallic behavior has for many decades confined this theoretical work to formal developments and unverified predictions. However, progress in synthesis and charac- terization techniques in the late 1970s allowed a con- frontation between theory and experiments. Besides these fundamental aspects, the technological interest in controlling the properties of nanosized and/or plastic conductors was a strong driver for exploring this field. The attribution of the chemistry Nobel prize in 2000 to A. J. Heeger, A. G. MacDiarmid, and H. Shirakawa for the “discovery and development of conductive poly- mers” was a clear recognition from the community of the importance, and the difficulty, of obtaining conju- gated one-dimensional metallic systems. Further, even when metallic, the conductivity in such systems has been shown to usually remain very low, with in most cases polaron-assisted transport leading to very large effective masses for the carriers. As a paradigmatic example, the conducting !and even superconducting" properties of DNA, at the frontiers of physics, chemistry, and biology, are currently generating fierce controversies in the lit- erature.

The field of nanotubes has strongly benefited from this broad fundamental and technological interest. Not only can nanotubes be metallic, they are also mechani-

cally very stable and strong, and their carrier mobility is equivalent to that of good metals, suggesting that they would make ideal interconnects in nanosized devices. Further, the intrinsic semiconducting character of other tubes, as controlled by their topology, allows us to build logic devices at the nanometer scale, as already demon- strated in many laboratories. Finally, the large fullerene community !yet another area recognized by the Nobel prize in chemistry in 1996", and the even larger family of researchers interested in carbon-based systems, natu- rally joined this novel and promising field. This merging of interests and communities can certainly explain the formidable success and burgeoning activity generated by the discovery of nanotubes in 1991.

A nanotube is a honeycomb lattice rolled into a hol- low cylinder with nanometric diameter and "m length. Depending on the community, specific interests, and tar- geted applications, nanotubes are regarded as either single molecules or quasi-one-dimensional crystals with translational periodicity along the tube axis. As there are an infinite number of ways of rolling a sheet into a cylinder, the large variety of possible helical geometries, defining the tube chirality, provides a family of nano- tubes with different diameters and microscopic struc- tures. Some properties of these nanotubes, such as the elastic ones, can be explained within a macroscopic model of a homogeneous cylinder. Others depend cru- cially on the atomic configuration. For instance, the elec- tronic and transport properties, which constitute the scope of the present review, are certainly among the most significant physical properties of carbon nanotubes, and crucially depend on the diameter and chirality. This dependence on the atomic configuration, an effect ex- plained below, is quite unique in solid-state physics. This sensitivity constitutes a challenge for synthesis tech- niques, since well-controlled properties are often de- sired, but it is also a source of innovation for applica- tions.

In the following sections, we show how carbon nano- tubes can be either !semi"metallic or semiconducting, with a band gap varying from zero to a few tenths of an eV, depending on their diameter and chirality. Further, the band gap of semiconducting tubes, or the energy difference between the peaks in the electronic density of states !the so-called van Hove singularities", can be shown to first order to be simply related to the tube diameter. Such remarkable results can be obtained from a variety of considerations, starting from the so-called band-folding approach, based on knowledge of the elec- tronic properties of the graphene sheet, to the direct study of nanotubes using semiempirical tight-binding ap- proaches. The comparison with more sophisticated ab initio calculations, and with available experimental re- sults, allows us to set the limits of these simple treat- ments, with the introduction of finer considerations, such as curvature or trigonal warping effects.

Knowledge of the electronic properties of nanotubes further permits one to study their response to external probes. This is a crucial issue as it conditions most of the potentiality for the integration of tubes in real devices

678 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

and allows us to relate the structural and electronic properties with the experimental optical, Raman, etc., spectra. In particular, the effect of a magnetic field on the electronic band structure, the optical absorption and emission spectra, and finally the transport properties of tubes will be presented.

The tremendous importance of the transport proper- ties of nanotubes, from both a fundamental and techno- logical point of view, justifies devoting the second part of this review to that subject. First, the main characteristics of ballistic transport will be clarified, followed by a few analytical results about the absence of backscattering in the presence of long-range disorder and the derivation of the elastic mean free path induced by short-range dis- order. All transport regimes will be reviewed in the pres- ence of elastic disorder, starting with the simple Ander- son model, followed by an extended analysis of more realistic disorders such as chemical substitutions or func- tionalization, topological defects, and so on. Quantum interference effects will then be addressed with a focus on weak- and strong-localization regimes, in light of re- cent experiments. Further, the contribution of inelastic scattering mechanisms !through electron-electron and electron-phonon interactions" will be scrutinized, with a discussion of the inelastic scattering times and decoher- ence mechanisms. As a specific case of transport !or tun- neling", with much technological importance, the physics of field emission from nanotubes will be briefly pre- sented.

Several topics strongly related to quantum confine- ment and dimensionality effects will be addressed at the end of this review. At the heart of the complex behavior of 1D systems, the physics of the Luttinger-liquid transi- tion will be highlighted and the signature of this transi- tion in available transport experiments will be put in perspective. Coulomb-blockade effects and their mani- festation in transport measurements will then be sum- marized. Finally, the competing charge-density-wave !or Peierls" and superconducting instabilities upon switching on the electron-phonon interaction, observed experi- mentally, will be discussed.

The contents of the present review are theoretical, and experimental results are used primarily to provide the necessary and crucial evidence for validation of the theory. As a matter of fact, the difficulty in performing the synthesis and characterization of well-defined and isolated nanotubes has on many occasions granted to theory the important, but also dangerous, role of predic- tion. In return, these experimental difficulties have fos- tered the elaboration of original and creative experi- mental techniques. As emphasized below, most of the theoretical predictions seem now to be confirmed by many experimental results.

Even with a focus on theoretical results, space limita- tions impose a drastic, and necessarily subjective, selec- tion of topics and references. Thorough lists of refer- ences and a more complete picture !with, e.g., a description of the synthesis and characterization tech- niques" can be found in the excellent books devoted to the subject !Dresselhaus et al., 1996, 2001; Endo et al.,

1996; Ebbesen, 1997; Saito et al., 1998; Harris, 1999; Tománek and Enbody, 1999; Reich et al., 2004; Loiseau et al., 2006".

II. STRUCTURE OF CARBON NANOTUBES

Carbon nanotubes were discovered and first charac- terized in 1991 by Iijima from NEC laboratories !Japan" !Iijima, 1991". This discovery was made possible thanks to the use of state-of-the-art transmission microscopy. The first nanotubes discovered were made of several concentric cylindrical-like shells regularly spaced by an amount of about 3.4 Å as in conventional graphite materials !Fig. 1, left". These multiwall nanotubes !MWNTs" were first synthesized with diameters ranging from a few nanometers to several hundred nanometers for the inner and outer shells, respectively. As for the length, MWNTs extending over several microns are cur- rently synthesized.

Shortly after the discovery of multiwall carbon nano- tubes, single-wall carbon nanotubes !SWNTs" were syn- thesized in abundance using arc-discharge methods with transition-metal catalysts !Bethune et al., 1993; Iijima and Ichihashi, 1993". A carbon nanotube made of a single graphite layer !the graphene sheet" rolled up into a hollow cylinder is called a single-wall nanotube. These tubes have quite small and uniform diameter, on the or- der of 1 nm=10!9 m. This unprecedentedly small diam- eter, combined with the crystalline perfection of the atomic network, explains why these objects were quickly considered as the ultimate carbon-based 1D systems.

Crystalline ropes !or bundles" of SWNTs, with each rope containing tens to hundreds of tubes of similar di- ameter, closely packed in a hexagonal configuration, have also been synthesized using a laser vaporization method !Guo et al., 1995" and arc-discharge and chemi- cal vapor deposition !CVD" techniques !Fig. 1, right". Various synthesis methods have provided ample amounts of sufficiently characterized samples for study- ing the fundamental properties of SWNTs.

Because the microscopic structure of SWNTs is closely related to that of graphene, the tubes are usually labeled in terms of the graphene lattice vectors. As illus- trated in Fig. 2 a single-wall carbon nanotube is geo- metrically obtained by rolling up a single graphene strip !Saito et al., 1998". Its structure can be specified or in- dexed by its circumferential vector !Ch", as defined by the chiral vector !AA! in Fig. 2" which connects two crystallographically equivalent sites !A and A!" on a graphene sheet. In this way, a SWNT’s geometry is com- pletely specified by a pair of integers !n ,m" denoting the relative position Ch=na1+ma2 of the pair of atoms on a graphene strip which, when rolled onto each other, form a tube !a1 and a2 are unit vectors of the hexagonal hon- eycomb lattice; see Fig. 2".

This chiral vector Ch defines the circumference of the tube. The diameter dt of the nanotube can thus be esti- mated from

679Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

dt = #Ch#/# = a #

$n2 + nm + m2, !1"

where a is the lattice constant of the honeycomb net- work: a=$3$acc !acc%1.42 Å, the C-C bond length". The chiral vector Ch uniquely defines a particular !n ,m" tube, as well as its chiral angle %, which is the angle between Ch and a1 !zigzag direction of the graphene sheet; see Fig. 2". The chiral angle % can be calculated as follows:

cos % = Ch · a1

2$n2 + nm + m2 . !2"

The value of % is in the range 0& #%#&30°, because of the hexagonal symmetry of the graphene lattice. This chiral angle % also denotes the tilt angle of the hexagons with respect to the direction of the nanotube axis. Nanotubes of the type !n ,0" !%=0° " are called zigzag tubes, because they exhibit a zigzag pattern along the circumference. Such tubes display carbon-carbon bonds parallel to the nanotube axis. Nanotubes of the type !n ,n" !%=30° " are called armchair tubes, because they exhibit an armchair pattern along the circumference. Such tubes display carbon-carbon bonds perpendicular to the nanotube axis. Both zigzag and armchair nanotubes are achiral tubes, in contrast with general !n ,m#n#0" chiral tubes !Fig. 3".

The geometry of the graphene lattice and the chiral vector determine not only the diameter of the tube, but also the unit cell and its number of carbon atoms. The smallest graphene lattice vector T perpendicular to Ch

FIG. 1. High-resolution transmission electron microscopy pictures of a multiwall carbon nanotube !left" and a bundle of single- wall nanotubes !right", illustrating two different possible geometries for nanotubes. Courtesy of Gavillet, 2001.

FIG. 2. Graphene honeycomb network with lattice vectors a1 and a2. The chiral vector Ch=5a1+3a2 represents a possible wrapping of the two-dimensional graphene sheet into a tubular form. The direction perpendicular to Ch is the tube axis. The chiral angle % is defined by the Ch vector and the a1 zigzag direction of the graphene lattice. In the present example, a !5,3" nanotube is under construction and the resulting tube is illustrated on the right.

FIG. 3. Atomic structures of !12,0" zigzag, !6,6" armchair, and !6,4" chiral nanotubes.

680 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

defines the translational period t along the tube axis. The lattice vector T can also be expressed in terms of the basis vectors a1 and a2 as T= t1a1+ t2a2. Using Ch ·T =0, the expressions for t1 and t2 are given by

t1 = 2m + n

, !3"

where NR is the greatest common divisor of !2m+n" and !2n+m". The length of the translational vector t is given by

t = #T# = $3a$n2 + nm + m2/NR. !4"

The nanotube unit cell is thus formed by a cylindrical surface with height t and diameter dt. The number of carbon atoms per unit cell NC can also be expressed as a function of n and m:

NC = 4!n2 + nm + m2"/NR. !5"

The symmetry of carbon nanotubes can be described by the so-called line groups, which are full space groups of one-dimensional systems including translations in addi- tion to the point-group symmetries like rotations or re- flections. The carbon-nanotube line groups are nonsym- morphic groups as they always contain a screw axis. Every !n ,m" carbon nanotube belongs to a different line group !Damnjanovic et al., 1999; Reich et al., 2004". Only

armchair !n ,n" and zigzag !n ,0" tubes with the same n belong to the same symmetry group. Moreover, by start- ing with a single carbon atom and successively applying all symmetry operations of the line group, the whole tube is constructed. However, for many applications, such as optical transitions or first-order Raman scatter- ing, it is not necessary to work with the full line group, the point group being quite sufficient. These point groups are Dq for chiral nanotubes !n ,m#n#0" and D2nh for achiral tubes such as !n ,n" or !n ,0". After the symmetry operations of the nanotube have been deter- mined using its point group and its most basic structural properties !diameter, chirality, lattice, and reciprocal lat- tice vectors, as summarized in Table I", the correspond- ing graphene strip can be constructed and rolled up into a cylinder. The next step is now to predict its electronic behavior.

III. ELECTRONIC PROPERTIES OF CARBON NANOTUBES

Carbon nanotubes are characterized by two types of bond, in analogy with graphene, which exhibits so-called planar sp2 hybridization. Among the four valence orbit- als of the carbon atom !the 2s, 2px, 2py, and 2pz orbitals, z perpendicular to the sheet", the !s ,px ,py" orbitals com- bine to form in-plane ' !bonding or occupied" and '*

TABLE I. Structural parameters for a !n ,m" carbon nanotube. In this table, n, m, t1, t2 are integers.

Symbol Name Formula Value

a lattice constant a=$3acc%2.46 Å acc%1.42 Å

a1, a2 basis vectors !$3 2

; 1 2 "a, !$3

$3 ;1"2#

a , ! 1

$3 ;!1"2#

a

Ch chiral vector Ch=na1+ma2&!n ,m" !0& #m#&n"

dt tube diameter dt=

2n+m

T translational vector T= t1a1+ t2a2&!t1 , t2" gcd!t1 , t2"=1a

t1= 2m+n

NC number of C atoms per unit cell NC=

4!n2+nm+m2" NR

agcd!n ,m" denotes the greatest common divisor of the two integers n and m.

681Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

!antibonding or unoccupied" orbitals !Fig. 4". Such orbit- als are even with respect to planar symmetry. The ' bonds are strong covalent bonds responsible for most of the binding energy and elastic properties of the graphene sheet. The remaining pz orbital, pointing out of the graphene sheet, is odd with respect to the planar symmetry and cannot couple with the ' states. The lat- eral interaction with neighboring pz orbitals !labeled the pp# interaction" creates delocalized # !bonding" and #*

!antibonding" orbitals. In analogy, the ' bonds in the nanotube form a hexagonal network which strongly con- nects the carbon atoms in the cylinder wall of the tube. The # bonds are perpendicular to the surface of the nanotube and are responsible for the weak interaction between SWNTs in a bundle, similar to the weak inter- action between carbon layers in pure graphite !Charlier et al., 1991". The energy levels associated with the in- plane ' bonds are known to be far away from the Fermi energy in graphite !Fig. 4, right" and thus do not play a key role in its electronic properties. In contrast, the bonding and antibonding # bands cross the Fermi level

at high-symmetry points in the Brillouin zone of graphene !Wallace, 1947". For a good understanding of the electronic properties of SWNTs, the electronic struc- ture of graphene will be briefly discussed in the next section.

A. From graphite to nanotubes

Although graphite has been studied for decades, graphene was only isolated experimentally in 2004 after a long struggle !Novoselov et al., 2004". Further, and de- spite early predictions !Wallace, 1947", its remarkable conducting properties, in which electrons mimic the be- havior of massless, relativistic particles, have only been observed recently !Novoselov et al., 2005; Zhang et al., 2005".

The electronic bands of graphene along the high- symmetry M-(-K directions are presented in Fig. 5. The # and #* bands cross at the vertices of the hexagonal Brillouin zone !Fig. 6". Such vertices are labeled by their momentum vector usually written as K. Consequently, graphene is a special semimetal whose Fermi surface is reduced to the six distinct K points of the hexagonal Brillouin zone. Close to the Fermi energy, the # and #*

bands are nearly linear, in contrast with the quadratic energy-momentum relation obeyed by electrons at band edges in conventional semiconductors. This linear energy-momentum relation of electrons will explain the extremely good conductivity in graphene and bears much importance in the Luttinger-liquid !LL" behavior for low-energy excitations in nanotubes !see Sec. IV.E.3".

The bonding and antibonding ' bands are well sepa- rated in energy !)10 eV at (". These bands are fre- quently neglected in semiempirical calculations as they are too far away from the Fermi level to play a role in the electronic properties of graphene. The remaining two # bands can be simply described with a rather simple tight-binding Hamiltonian, leading to analytical solutions for their energy dispersion and the related eigenstates. This simple approach can be further ex-

FIG. 5. Electronic properties of graphene. !a" Electronic band structure of graphene. The bonding ' and antibonding '* bands are separated by a large energy gap. The bonding # !last valence" band and antibonding #* !first conduction" band cross at the K points of the Brillouin zone. The Fermi energy is set to zero, and * indicates the work function. Above the vaccuum level !dotted horizontal line", the states of the continuum are difficult to describe and merge with the '* bands. !b",!d" # state at K and !c",!e" ' state at (, seen from above and from the side of the graphene plane. Note that the # wave function cancels on a hexagonal sublattice due to the exp!iK ·r" phase factor. The # !'" state is odd !even" with respect to the graphene plane reflection. Courtesy of Fernández-Serra, 2006.

FIG. 4. The ' bonds in the carbon hexagonal network connect the carbon atoms and are responsible for the binding energy and the elastic properties of the graphene sheet !left". The # bonds are perpendicular to the surface of the sheet. The cor- responding bonding and antibonding ' bands are separated by a large energy gap !right", while the bonding and antibonding # states lie in the vicinity of the Fermi level !EF". Adapted from Loiseau et al., 2006.

682 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

tended to study the properties of nanotubes by combin- ing these analytic results with the requirement that the wave functions in tubes must satisfy the proper bound- ary conditions around the tube circumference. This is what we show in the next sections.

B. Tight-binding model of graphene

As mentioned in the previous section, the graphene plane is a hexagonal lattice with two atoms per unit cell !A and B" and a basis defined by vectors !a1 ,a2" !see Fig. 6". The condition ai ·bj=2#+ij allows one to obtain the reciprocal-lattice vectors !b1 ,b2". Every carbon atom possesses four valence electrons !two 2s and two 2p elec- trons". When the atoms are placed onto the graphene hexagonal lattice, as in Fig. 6, the electronic wave func- tions from different atoms overlap. However, such an overlap between the pz orbitals and the s or px and py electrons is strictly zero by symmetry. Consequently, the pz electrons, which form the # bonds in graphene, can be treated independently of other valence electrons. Within this #-band approximation, the A atom !B atom" is uniquely defined by one orbital per atom site pz!r !rA" 'pz!r!rB"(.

To derive the electronic spectrum of the total Hamil- tonian, the corresponding Schrödinger equation has to be solved, and by applying the Bloch theorem, the wave functions can be written as follows:

,!k,r" = cA!k"pz A!k,r" + cB!k"pz

eik·!pz!r ! rB ! !" , !8"

where k is the electron momentum !the quantum num- ber", Ncells is the number of unit cells in the graphene sheet, and ! is the cell position index. The spectrum is derived by solving the Schrödinger equation which re- duces to a 2$2 matrix diagonalization:

*HAA ! E HAB

HAA!k" = 1

A,!!- , !10"

HAB!k" = 1

B,!!- , !11"

with the notation pz A/B,-=pz!r!rA/B!-". Here we have

neglected the overlap matrix elements S= ,pz A # pz

B- be- tween neighboring pz orbitals !neglect of overlap inte- grals defines the so-called orthogonal tight-binding schemes". After simple manipulations and restricting in- teractions to first nearest neighbors only, one gets

HAB!k" = ,pz A,0#H#pz

B,0- + e!ik·a1,pz A,0#H#pz

B,!a1-

B,!a2- = ! .0/!k" , !12"

with .0 the transfer integral between first-neighbor # orbitals !a typical value for .0 is 2.9 eV", /!k"= !1 +e!ik·a1 +e!ik·a2", and ,pz

A,0#H#pz A,0-= ,pz

B,0#H#pz B,0-=0 as

the energy reference. The dispersion relations are then readily obtained:

E±!k" = ± .0$3 + 2 cos!k · a1" + 2 cos!k · a2" + 2 cos'k · !a2 ! a1"( , !13"

which can be further developed as

E±!kx,ky" = ± .0$1 + 4 cos $3kxa

2 cos

kya 2

!14"

by setting a=$3acc !acc=1.42 Å". The k= !kx ,ky" vectors that belong to the first hexagonal Brillouin zone !BZ"

constitute an ensemble of available electronic momenta. In Fig. 7, these simple tight-binding dispersion relations are represented with dashed lines along high symmetry directions of the BZ, defined by the ( and M points together with the six BZ vertices !K points".

With one pz electron per atom in the #-#* model !the three other s, px, and py electrons fill the low-lying ' band", the !!" band !negative energy branch" in Eq. !14"

FIG. 6. Brillouin zone and reciprocal space. !a" Basis vectors in the hexagonal lattice of graphene. !b" Brillouin zone. The corresponding reciprocal basis vectors read b1=b!1/2 ,$3/2" and b2=b!1/2 ,!$3/2", with b=4# /a$3.

683Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

is fully occupied, while the !0" branch is empty. These occupied and unoccupied bands cross at the K points 'one verifies that /!k=K"=0(. The Fermi level EF !or charge-neutrality point" is therefore the zero-energy ref- erence in Fig. 7, and the Fermi surface is defined by the set of K points. Since the occupied and unoccupied bands do cross, the graphene sheet displays a metallic !zero-gap" character. However, as the Fermi surface is of zero dimension !since it is reduced to a discrete and fi- nite set of points", the term semimetal is usually used.

This simple orthogonal tight-binding model yields # and #* zone-center ( energies which are symmetric !±.0" with respect to EF. In fact, the antibonding !unoc- cupied" #* bands are located at a higher energy if the overlap integral S is not set to zero !see Fig. 7". A better, but more complicated, #-#* parametrization can be found in Reich, Maultzsch, Thomsen, and Ordejón !2002" where a careful comparison between ab initio and various tight-binding schemes is presented for graphene and several nanotubes. The main advantage of the present nearest-neighbor approximation is the very simple analytical expression for the # electronic states of graphene.

C. Zone-folding approximation

Due to periodic boundary conditions along the cir- cumferential direction of the tube, the allowed wave vectors “around” the nanotube circumference are quan- tized: they can take only a set of discrete values. In con- trast, the wave vectors along the nanotube axis remain continuous !for infinite tubes". Plotting these allowed vectors for a given nanotube onto the Brillouin zone of graphene generates a series of parallel lines. The length, number, and orientation of these cutting lines depend on the chiral indices !n ,m" of the nanotube. The basic idea behind the zone-folding approximation is that the elec-

tronic band structure of a specific nanotube is given by superposition of the graphene electronic energy bands along the corresponding allowed k lines. This is what we explain now.

A specific carbon nanotube defines a unique chiral vector Ch= !n ,m" expressed in the basis !a1 ,a2" !Fig. 2" that fixes its symmetry and its diameter. As mentioned in Sec. II, the chiral vector length #Ch# equals $3acc$n2+nm+m2 or #dt !dt being the nanotube diam- eter". The application of periodic boundary conditions around the tube circumference leads to some restrictions on the allowed wave function quantum phase:

,k!r + Ch" = eik·Ch,k!r" = ,k!r" , !15"

with the vectors r and k taken on the tube surface. The first equality stems from the Bloch theorem. Depending on the tube symmetry, that is, on the chiral vector Ch = !n ,m", two situations can occur.

1. Metallic nanotubes

We make an analysis in the neighborhood of the Fermi surface, so that we write k=K++k, with +k small, taking, e.g., K= !b1!b2" /3= !0,4# /3a", so that k = !+kx ,4# /3a++ky". When eiK·Ch =1 !which is possible only when n!m=3l, with l an integer", then the con- straint on the wave function becomes +k ·Ch=2#q !q in- teger". Each index q defines a line of allowed k vectors, and each line contributes to one occupied # band and one unoccupied #* band. The condition n!m=3l is al- ways satisfied for armchair tubes and for the subset of the !n ,0" zigzag tubes with n multiples of 3. Rewriting the dispersion relation in the general case as E2!kx ,ky" =.0

2#/#2 and performing a second-order perturbation ex- pansion in the vicinity of the K points, one finally ob- tains #/!kx ,ky"#2% 3

4 !+kx 2++ky

2"+O!+k3" !with +kx and +ky related by +k ·Ch=2#q". Close to EF, the dispersion re- lation then reads E±!+k"% ± !$3a /2".0.+k., a linear energy-momentum relation mentioned above. There- fore, states arbitrarily close in energy to the Fermi level can be found for q=0 and the system is metallic !see Fig. 8". The Fermi velocity vF=$3a.0 /21= 3

2acc.0 /1 is typi- cally given by vF%8$105 m s!1 for .0=2.9 eV. The lin- ear band dispersion close to EF will be shown to have useful consequences.

A simple expression for the eigenstates can also be derived close to EF within the same type of approxima- tion. Such an expression will be used in Sec. IV.C.2 to show that elastic backscattering is quenched in nano- tubes if the disorder is long ranged. One notes that, for a general helical symmetry, the full properties of the eigenstates can be derived by constructing generalized Bloch states satisfying helical !rototranslation" symme- tries !Mintmire et al., 1992".

2. Semiconducting nanotubes

The second possible choice for !n ,m" nanotubes is given by the condition n!m=3l±1. In this situation

FIG. 7. Limitations of the #-#* model. !a" Ab initio !solid lines" and nearest-neighbor orthogonal tight-binding 'dashed lines, from Eq. !14"( # and #* electronic bands for graphene. !b" Difference 2E between the ab initio and tight-binding band structures. Adapted from Reich, Maultzsch, Thomsen, and Or- dejón, 2002.

684 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

eiK·Ch = ±e2i#/3, and one gets +k= !2# / #Ch#"!q±1/3"3!

+k.3. with 3! and 3. the basis vectors along the Ch and T directions, respectively, where T is the translational vector along the tube axis, as defined in Sec. II. By fol- lowing a similar calculation as for the prior case, one obtains in the vicinity of the Fermi level a new disper- sion relation, namely,

Eq ±!k." % ±

+ k. 2, !16"

where the integer variable q counts the available bands, whereas k. is the part of the wave vector that continu- ously describes the states within a given subband !and associated with the direction parallel to the tube axis".

This case leads to an obvious gap opening at the Fermi level !Fig. 9" since

Eq=0 + !k. = 0" ! Eq=0

! !k. = 0" = 2#a.0

1. !17"

It appears that 2Eg 1 decreases as the inverse of the tube

diameter dt !dt= #Ch# /#". For a very large diameter, one finds as expected a zero-gap semiconductor since we re- cover the graphene sheet. For realistic tubes, with, e.g., a diameter of 1.4 nm 'helical vector !17,0"(, one gets 2Eg

1

%0.59 eV. This 1 /d dependence of the gap on the diam- eter relies on the assumption of a linear dispersion of the bands around EF, a result first derived by White and Mintmire !1998". In reality, the bands are not linear away from EF, an effect called trigonal warping !Saito, Dresselhaus, and Dresselhaus, 2000" which induces a de- pendence of the band gap not only on the diameter, but on the !n ,m" indices as well.

In relation to the study of transport properties an im- portant quantity linked to the dispersion relation is the so-called effective mass of the charge carriers. In semi- conducting nanotubes, this quantity can be derived from Eq. !16",

Eq=0 ± = ± $!m*vF

2"2 + !1k.vF"2,

defining m*=2#1 /3#Ch#vF, which is thus inversely pro- portional to the nanotube diameter and tends to zero as the diameter tends to infinity !graphene limit". This con- cept has been used !Zhou et al., 2005" to estimate the charge mobility properties in semiconducting nanotubes.

In summary, early theoretical calculations !Hamada et al., 1992; Mintmire et al., 1992; Saito et al., 1992" showed that the electronic properties of carbon nanotubes are very sensitive to their geometric structure. Although graphene is a semimetal, theory has predicted that car- bon nanotubes can be metals or semiconductors with an energy gap that depends on the tube diameter and he- licity, i.e., on the indices !n ,m". These results can be simply understood within a band-folding picture, as il- lustrated in the present section. This approach is made relatively simple in nanotubes because of the special shape of the graphene Fermi surface and the restriction of the electronic bands to the #-#* manifold.

FIG. 8. The band-folding scheme. !a" Brillouin zone of graphene. The white rectangle is the Brillouin zone associated with the four-atom cell with lattice vectors Ch /n=a1+a2 and T !T=a1!a2 for an armchair tube". Thick lines are the allowed k lines for the !5,5" armchair tube. To obtain the !5,5" band struc- ture in the band-folding approach, fold the colored corners onto the rectangular cell and superimpose the graphene energy bands calculated along the obtained thick lines of length 2# / #T#. In particular, the K points are folded at two-thirds of (X !or its inversion symmetry image". The bands are indexed by the integer q such that k ·Ch=2#q. In the corresponding !5,5" tube, q is also the azimuthal quantum number. !b" Disper- sion relations E±!kx ,ky" for the graphene plane, together with that of an armchair nanotube !bold line".

FIG. 9. Dispersion relations E±!kx ,ky" for the graphene plane, together with that of a zigzag semiconducting nanotube !bold line".

685Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

When forming a tube, owing to the periodic boundary conditions imposed in the circumferential direction, only a certain set of k vectors in the graphene BZ are al- lowed. This allowed set of Bloch momenta depends on the diameter and helicity of the tube. Whenever the al- lowed k vectors include the point K, the system is a metal with a nonzero density of states at the Fermi level, resulting in a one-dimensional metal with two bands dis- persing linearly close to EF. When the K point is not included, the system is a semiconductor with a small band gap that depends mainly on the diameter. In this case, the conduction- and valence-band edges come from states with k vectors located on the allowed line!s" closest to the K point.

Within the zone-folding approximation, the general rules for the metallicity of single-wall carbon nanotubes are as follows: a nanotube defined by the !n ,m" indices will be metallic !semiconductor" if n!m=3l, with l an integer !n!m=3l±1". Consequently, most carbon nano- tubes are semiconductors and only a fraction !1/3" are metallic !or semimetallic".

To conclude this subsection, we note that the index q, as defined above by the condition k ·Ch=2#q 'Eq. !15"( is also the azimuthal quantum number associated with the states on the corresponding allowed k line. This quantum number therefore characterizes the behavior of eigenstates with respect to rotations around the axis that transform the tube into itself. It can be used in par- ticular to study, on the basis of symmetry-related selec- tion rules !Vucovic et al., 2002", the effect of a perturba- tion on various subbands and their mixing upon static !e.g., tube squashing, interaction with a substrate, etc." or time-dependent !e.g., optical excitation" perturba- tions.

D. Band structures and densities of states

As the nanotubes are one dimensional, their Brillouin zone is one dimensional as well, with zone edges usually labeled X, namely, X= ± !# /T"!., with !. and T defined above. The nanotube band structure is therefore repre- sented along the (X direction !(X! with X!=!X sym- metric by time reversal". In the band-folding approach, one obtains therefore a superposition of all allowed Eq

±!k." graphene eigenvalues, with q the allowed line in- dex !two bands per line" and k. the continuous momen- tum along 3. !from now on, as there is only one direc- tion, we drop the . subscript and write k. =k". One says that the allowed k lines are “folded” onto the (X direc- tion 'see Fig. 8!a" for armchair tubes(. We now study the band structure and related density of states of !n ,m" tubes as given by the band folding of the #-#* bands of graphene within the orthogonal tight-binding scheme presented above.

The electronic band structure of an armchair !5,5" car- bon nanotube is presented in Fig. 10. Six bands for the conduction and an equal number for the valence states are observable. However, four of them are degenerate, leading to ten electronic levels in each case, consistent

with the ten hexagons around the circumference of the !5,5" nanotube. Indeed, the bands coming from two al- lowed lines with opposite q index, for q= ±1 to q= ±4 'see Fig. 8!a"(, are degenerate by symmetry. For all arm- chair nanotubes, the energy bands exhibit a large degen- eracy at the zone boundary, where k= ±# /a !X point", so that Eq. !14" becomes E!k= ±# /a"= ±.0. This comes from the absence of dispersion along the segments con- necting the neighboring centers of the BZ sides !the M points", an effect that will yield the so-called trigonal warping of the bands as discussed below. The valence and conduction bands for armchair nanotubes cross at k=kF= ±2# / !3a", a point that is located at two-thirds of (X 'Fig. 8!a"(. This means that the original K vertices of the original graphene hexagonal BZ are folded at two- thirds of the (X line !or its inversion symmetry image". As discussed above, the !5,5" armchair nanotube is thus a zero-gap semiconductor which will exhibit metallic conduction at finite temperatures, since only infinitesi- mal excitations are needed to promote carriers into the conduction bands.

The density of states !DOS" 2N /2E represents the number of available states 2N for a given energy inter- val 2E !2E!0". This DOS is a quantity that can be measured experimentally under some approximations. The shape of the density of states is known to depend dramatically on dimensionality. In 1D, as shown below, the density of states diverges as the inverse of the square root of the energy !1/$E" close to band extrema. These “spikes” in the DOS are called Van Hove singularities !VHSs" and manifest the confinement properties in di- rections perpendicular to the tube axis. As carbon nano- tubes are one dimensional, their corresponding DOSs exhibit such a spiky behavior at energies close to band edges !see Fig. 10". The position of these Van Hove sin- gularities can be analytically derived from the dispersion relations. The density of states is defined by

FIG. 10. Band structure and density of states for a !5, 5" arm- chair nanotube within the zone-folding model. The 1D energy dispersion relations are presented in the '!3.0 ;3.0( energy in- terval in dimensionless units !.0 being the nearest-neighbor C-C tight-binding overlap energy /2.9 eV". The energy bands are plotted along the X-(-X direction. The Fermi level is lo- cated at zero energy.

686 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

4!E" = 1 5

Tr'+!E ! H"( , !18"

where +!E!H" is the spectral measure; the trace is ex- panded within a complete basis, and 5 is the volume of the considered system. For the set of eigenvalues Eq

s !k", where s=± refers to the sign of the solution in Eq. !14", the DOS can be expressed as

4!E" = 2 5

= 2 5

$k 1!1

, !19"

where kqs are the roots of the equation E!Eq s !k"=0,

while 5=4##Ch# /$3a2 is the volume !surface" of the re- ciprocal space for each allowed state divided by the dis- tance between allowed lines in the graphene Brillouin zone !see above". In the vicinity of K, where one can use the linear energy-momentum relation, the contribution of k to the density of states is related to

1 $Eq s !k"

2 , !20"

where 6qs gives the energy position of the Van Hove singularities. In the vicinity of EF, those positions are given by #6qs#=$3.0a2k!

q /2 with 2k! q = 2!k!K" ·Ch / #Ch#2

=2##3q!n+m# /3#Ch#. Hence #6qs#=#.0acc#3q!n +m# / #Ch#, and one finally obtains the density of states

4!E" = 2a

2 . !21"

For all metallic nanotubes, the density of states per unit length along the nanotube axis is a constant at the Fermi energy !EF" and can be expressed analytically !Mintmire and White, 1998":

4!6F" = 2$3acc/!#.0#Ch#" . !22"

Beyond the linear-band approximation, one can rewrite Eq. !14" for metallic armchair !n ,n" nanotubes to obtain the following band dispersion relation:

Eq ±!k" = ± .0$1 + 4 cos

ka 2

, !23"

where q=1,2n corresponds to the discrete part of the wave vector !band index" and k is the continuous part of the wave vector, describing states in a specific band !!#7ka7#". The positions of the Van Hove singulari- ties can then be derived analytically directly from Eq. !23", and a simple calculation gives 6q,s=±= ±.0 sin q# /n. In Fig. 10, the spikes in the DOS are localized at 6q=1,10;s=±= ±.0 sin q# /5.

We now turn to zigzag tubes. The calculated 1D dis- persion relations E!k" for the !9,0" and !10,0" zigzag nanotubes are illustrated in Figs. 11 and 12, respectively. As expected, the !9,0" tube is metallic, with the Fermi surface located at (, whereas the !10,0" nanotube exhib-

its a finite energy gap at (. In particular, in the case of the !10,0" nanotube, there is a dispersionless energy band at E /.0= ±1, which gives a singularity in the DOS at these particular energies. For a general !n ,0" zigzag nanotube, when n is a multiple of 3, the energy gap at k=0 !( point" becomes zero. However, when n is not a multiple of 3, an energy gap opens at (. The correspond- ing densities of states have a zero value at the Fermi energy for the semiconducting nanotube and a small nonzero value for the metallic one.

It should be noted that the k values for the band crossing at EF in metallic nanotubes are k= ±2# /3T or k=0 for armchair or zigzag tubes, respectively. These k values are also the locations of the band gaps for semi- conducting zigzag nanotubes. The same k values denote as well the positions of the energy gaps !including zero energy gaps" for the general case of chiral nanotubes. In Fig. 13, the dispersion relations E!k" for the !8,2" chiral nanotube are shown. Since n!m is a multiple of 3, this nanotube exhibits a metallic behavior with a band cross- ing at k= ±2# /3T. Other chiral nanotubes, like the !9,6", display a zero energy gap at k=0. The DOS of chiral

FIG. 11. Band structure and density of states for a !9, 0" zigzag nanotube within the zone-folding model. The Fermi level is located at zero energy.

FIG. 12. Band structure and density of states for a !10,0" zigzag nanotube within the zone-folding model. The Fermi level is located at zero energy.

687Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

nanotubes !see Fig. 13" also displays Van Hove singulari- ties as for achiral tubes !Charlier and Lambin, 1998; Mintmire and White, 1998; White and Mintmire, 1998".

In semiconducting zigzag or chiral nanotubes, the band gap 'as expressed by Eq. !17"( is independent of the chiral angle and varies inversely with the nanotube diameter: 2Eg

1=2.0acc /dt !in the linear-band approxima- tion". Density-of-states measurements by scanning tun- neling spectroscopy !STS" provide a powerful tool for probing the electronic structure of carbon nanotubes. It can be shown, indeed, that under some assumptions the voltage-current derivative dI /dV is proportional to the DOS. These experiments !Odom et al., 1998; Wildöer et al., 1998" confirmed that the energy band gap of semi- conducting tubes is roughly proportional to 1/dt and that about 1/3 of nanotubes are conducting, while the other 2/3 are semiconducting. Resonances in the DOS have also been observed experimentally !Odom et al., 1998; Wildöer et al., 1998" on both metallic and semicon- ducting nanotubes whose diameters and chiral angles were determined using a scanning tunneling microscope !STM" !Venema et al., 2000". Several other experimental techniques, such as resonant Raman scattering !Jorio et al., 2001" and optical absorption and emission measure- ments !Bachilo et al., 2002; O’Connell et al., 2002; Le- febvre et al., 2003", have also confirmed this structure in Van Hove singularities of the electronic densities of states in single-wall carbon nanotubes.

E. Band structures in a magnetic field

The application of a uniform external magnetic field has profound consequences on the electronic band struc- ture of carbon nanotubes. There exist two cases of high symmetry for the direction of the magnetic field with respect to the nanotube axis. When the magnetic field is applied parallel to the tube axis, electrons within the nanotube are influenced by the electromagnetic poten- tial, whose dominating effect is to add a new phase fac- tor to the quantum wave function !with subsequent modification of the associated momentum", and in the

cylinder geometry this phase factor will be driven in a periodic fashion by the magnetic flux threading the nanotube cross section. This quantum phenomenon was first described theoretically by Aharonov and Bohm !1959", whereas field-periodic oscillations of the magne- toresistance were experimentally measured in ordinary metallic rings !Webb et al., 1985", opening a new field for mesoscopic physics !Imry, 1997".

Given that the metallic or semiconducting character of carbon nanotubes results from the existence of the allowed momentum k at the K points of the hexagonal Brillouin zone, the superimposed Aharonov-Bohm phase factor, modulated by the field, will induce some field-dependent disruption of the initial eigenstate distri- bution in reciprocal space, with a first spectacular effect of the band gap opening for an initially metallic system, as first described by Ajiki and Ando !1993". In this sec- tion, we provide the basics for understanding the Aharonov-Bohm phenomenon in carbon nanotubes and its consequences on the electronic spectrum. In Sec. IV.D.1, its corresponding effects on transport properties will be further described.

1. Aharonov-Bohm quantum phase

To further deepen and illustrate these effects, let us describe the modifications of the quantum phase factor, driven by the vector potential A and associated with the external magnetic field B=B!ux ,uy ,uz" !with B=rotA". Within the tight-binding scheme, the Bloch functions in the static B can be written as

,!k,r" = 1

$N ) R

eik·Rei8R9!rR" .

With R a lattice vector and 8R the phase factor associ- ated with the magnetic field, it can be shown that 8R!r" =3R

r A!r!"dr!=30 1!r!R" ·A!R+:'r!R("d: !Luttinger,

1951", so that the total matrix elements of H= !p /2m !eA"2+V!r", in the presence of B, are simply obtained through multiplication of those in the zero-field case by the phase factor !Saito et al., 1998". For a general de- scription of the B-dependent band-structure effects, one possibility is to adopt the Cartesian basis !ex ,ey ,ez" where ez and ex are, respectively, taken along and per- pendicular to the tube axis. In the Landau gauge A =B!0,uzx ,uxy", the Aharonov-Bohm phase acquired during an electronic motion between an orbital located at !xi ,yi ,zi" and another located at !xj ,yj ,zj" can be eas- ily derived:

8ij = 2# *0

2 5 , !24"

where *0 is the quantum flux. This result is applicable whatever the direction of B with respect to the tube axis and gives the axial configuration for !ux=0,uz=1" and the perpendicular configuration for !ux=1,uz=0". This further allows us to compute the remormalized field- dependent coupling overlap between # orbitals, .ij!B"

FIG. 13. Band structure and density of states for a !8,2" chiral nanotube within the zone-folding model. The Fermi level is located at zero energy.

688 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

=.0 exp'!2i# /*0"3ri

2. Parallel field: The band-gap opening and orbital degeneracy splitting

In the axial case, however, the use of another basis set makes understanding of the Aharonov-Bohm effect straightforward. Indeed, if one considers the two- dimensional Cartesian coordinates r= !x , y" in the basis defined by the directions !Ch ,T", then the vector poten- tial is recast as A= !* / #Ch# ,0" and the magnetic phase factor between two # orbitals located at ri= !xi , yi" and rj= !xj , yj" is simply written as 8i!8j= i*!xi! xj" / #Ch#. Ac- cordingly, the periodic boundary conditions on the quan- tum phase will be modified as

,k!r + #Ch#" = eik·Chexp*!2#/*0"0 r

r+Ch

A!r!"dr!+,k!r" ,

and since the additional magnetic phase factor thus re- duces to 2#* /*0, the change in the quantum momentum becomes

3! ! 3!!*" = 2# #Ch# *q ±

/

*0 + , !25"

with /=0 for metallic tubes, and /= ±1 for semiconduct- ing tubes. In Fig. 14 the effect of this change in momen- tum is illustrated in reciprocal space. From Eqs. !16" and !25", the field-dependent gap oscillation for an initially metallic tube is obtained,

2EB = Eq=0 + !k.,*/*0" ! Eq=0

! !k.,*/*0" = 32Eg 1*/*0,

if *&*0 /2, where 2Eg 1=2#acc.0 /$3#Ch# denotes the gap

at zero flux as given by Eq. !17". If *0 /2&*&*0, then 2EB=32Eg

1#1!* /*0#, so that the band gap exhibits an

oscillation between 0 and 2Eg 1 with a period *0 !Ajiki

and Ando, 1993, 1994, 1996; Tian and Datta, 1994; Lin et al., 1995; Lu, 1995". For instance, 2EB675 meV at 50 T for the !22,22" tube !diameter63 nm", while 2EB 640 meV at 60 T for the !10,10" tube !diameter =1.4 nm". In addition, to obtain a field equivalent to * =*0 in nanotubes with diameters of 1, 10, 20, and 40 nm, one typically needs magnetic fields of 5325, 53, 13, and 3 T, respectively.

In addition to such *0-periodic band-gap oscillations, the Aharonov-Bohm effect more generally affects the whole subband structure, as evidenced by Van Hove sin- gularity splitting and shifts !Jiang et al., 2000; Roche et al., 2000; Shyu et al., 2003". These effects result from the influence of the magnetic field on the orbital degeneracy. Indeed, the initial symmetry of the carbon nanotubes implies that each available energy level is initially four- fold degenerate !including spin and orbital degeneracy". The orbital degeneracy is attributed to the symmetry between clockwise !0" and counterclockwise !!" elec- tronic motions around the tube. In the presence of an external magnetic field, electrons in degenerate !0" and !!" eigenstates will acquire opposite orbital magnetic moments ±"orb, which will thus produce an upshift of the energy of !0" and a downshift of the energy of !!", resulting in lifting the orbital degeneracy !or Van Hove singularity splitting".

This mechanism is illustrated in the DOS plots for the !5,5" and !10,10" tubes in Figs. 15 and 16, respectively, which are both metallic nanotubes at zero magnetic field !Roche et al., 2000". The calculations have been per- formed using a simple tight-binding model in the #-orbital approximation, while nearest-neighbor hop- ping integrals have been renormalized in the presence of a magnetic field using Eq. !24".

FIG. 14. Representation of the first Brillouin zone of a graphene sheet together with allowed states for an armchair tube !dashed lines" at zero flux. Modifications of allowed states in the vicinity of k points, under the effect of a magnetic field applied parallel to the tube axis !circles give the equipotentials close to the Fermi energy".

FIG. 15. !Color online" Density of states of the !5,5" carbon nanotube for several magnetic flux values: * /*0=0 !a", * /*0 =0.1 !b", * /*0=0.2 !c", and * /*0=0.5 !d". This is a metallic tube at zero magnetic flux but a gap opens up once a finite flux is applied and increases with the flux.

689Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

As predicted theoretically, by applying a finite mag- netic flux * threading the tube, the band gap opens and increases linearly with *, to reach a maximum value at half the quantum flux !*0 /2". Further, the band gap is linearly reduced until it finally closes back when the field reaches one quantum flux. The labels !a"–!e" in Fig. 16 are the DOSs for the !10,10" tube at * /*0= !a" 0, !b" 0.125, !c" 0.25, !d" 0.375, and !e" 0.5. For * /*0=0.125 'trace !b"(, one notices that in the vicinity of the charge- neutrality point !i.e., 6=0", a new VHS appears, indicat- ing the gap opening. In !c", !d", and !e", the gap is seen to increase, reaching its maximum value at * /*0=0.5. The evolution of the VHS is then reversed and the gap closes again at * /*0=1. For VHSs at higher energies !e.g., those located at 6q=1", the oscillatory behavior is slightly more involved: at low fields a splitting is observed for each VHS, which is followed by crossing at higher flux, and finally all VHSs return to the original positions when * /*0=1 !see the inset of Fig. 16".

In the case of armchair !n ,n" metallic tubes, the mag- nitude of the field-dependent splitting of the qth VHS can be analytically ascertained:

2EB!6q,*/*0" = 2.04sin #

q*0 5 . !26"

Semiconducting tubes 'i.e., !n ,m" tubes with n!m =3l±1 !l being an integer"( are affected in a similar way, but the gap expression is slightly different. One finds 2EB=2Eg

1#1!3* /*0# if 0&*&*0 /2 and 2EB=2Eg 1#2

!3* /*0# when *0 /2&*&*0. Hence, the initial zero- field energy gap !2Eg

1" continuously decreases with in- creasing *, to reach zero at *=*0 /3. The gap further opens as * increases from *0 /3, reaching a local maxi-

mum !2Eg 1 /2" at *=*0 /2, before closing again at *

=2*0 /3, and finally recovering its original value 2Eg 1 at

*=*0. In Fig. 17, the DOS of a 3-nm-diameter semicon- ducting single-walled tube for various magnetic flux is illustrated. One notes that magnetic-field-induced lifting of the spin degeneracy brings some additional contribu- tion to the total electron magnetic moment !Zeeman ef- fect". This effect has been shown to yield an energy level displacement between spin up and spin down, linear with the magnetic flux, but inversely proportional to the squared radius of the tube !Jiang et al., 2000".

The Van Hove singularity splitting was recently ob- served by spectroscopic experiments !Zaric et al., 2004". In addition, several experimental studies of electronic transport spectroscopy at low temperature in the Cou- lomb blockade regime !Kanda et al., 2002; Coskun et al., 2004; Jarillo-Herrero et al., 2004; Minot et al., 2004" or in the Fabry-Perot regime !Cao et al., 2004; Jarillo-Herrero et al., 2005" have also provided compelling evidences of the Aharonov-Bohm effect. The experimental estima- tion of the orbital magnetic moment was found to be of the order of %0.7–1.5 meV/T !Minot et al., 2004; Jarillo-Herrero et al., 2005".

Magnetoresistance oscillations were also a subject of intense controversy in the early stage of carbon nano- tube studies, since the origin and value of the Aharonov- Bohm oscillation period were apparently of different na- tures. Indeed, while some studies of large-diameter multiwall carbon nanotubes !Bachtold et al., 1999" first revealed clear signatures of weak localization, with negative magnetoresistance and !*0 /2"-periodic Aharonov-Bohm oscillations driven by quantum inter- ferences !Altshuler and Aronov, 1985", other reports as- signed their magnetoresistance oscillations to field- modulated band structure effects, assuming a negligible contribution from interference effects !Fujiwara et al., 1999; Lee et al., 2000". The superimposed contributions to the Aharonov-Bohm oscillations from both band- structure and quantum interferences effects have been clearly disentangled recently !Stojetz et al., 2005" and will be discussed in Sec. IV.D.1.

FIG. 16. Density of states of the !10,10" metallic tube as a function of energy for several magnetic flux values !see text". Curves have been vertically offset for clarity. Inset: Evolution of one VHS with magnetic flux. Adapted from Roche et al., 2000.

FIG. 17. Density of states of the !21,23" tube at zero and finite flux. Top inset: Expanded plot of the DOS. Bottom inset: Evo- lution of the VHS splitting 2B as a function of magnetic field.

690 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

3. Perpendicular field: The onset of Landau levels

In the situation where the magnetic field is applied perpendicular to the tube axis, the modifications of the electronic spectrum are profoundly different. First the two-dimensional vector potential within the Landau gauge for the nanotube surface is now given by A = „0, !#Ch#B /2#"sin!2#x / #Ch#"…, keeping !x , y" as the co- ordinates along the circumferential and nanotube axis directions. For evident symmetry reasons, the net mag- netic flux threading the tube is now zero. The phase fac- tors can be computed using either this basis or the Car- tesian basis defined earlier. The energy dispersion can then be evaluated as a function of magnetic field inten- sity !Ajiki and Ando, 1993, 1996; Saito et al., 1994". In Fig. 18, the dispersion relation of the energy E /.0 is reported as a function of the dimensionless wave vector k.#T# /2# !Saito et al., 1994", for several values of the dimensionless inverse magnetic length ;= #Ch# /2#!m, where !m=$1 /eB is the magnetic length !first cyclotron orbit radius".

As seen in Fig. 18, as the intensity of the magnetic field is enhanced, the subband dispersion is reduced, with a particularly strong effect in the vicinity of the charge-neutrality point. This onset of a Landau-type subband can be further rationalized analytically. Indeed, by using the k ·p method, an expression for the eigen- states under magnetic field close to the K points can be derived analytically for metallic tubes !see Sec. IV.C.1

for the zero-field case". The k ·p equation at the charge- neutrality point !"k=0" in the presence of a perpendicu- lar magnetic field can be decoupled into two equations !Ando and Seri, 1997":

4! $

$x +

k !x" = 0, !27"

k !x" = 0, !28"

,A!x" = *1 0 +FA!x", ,B!x" = *0

1 +FB!x" ,

FA!x" = 1

#Ch# +5 ,

FB!x" = 1

#Ch# +5 ,

where I0!2;2" is a modified Bessel function of the first kind. Note that for sufficiently large magnetic field !; <1" these wave functions become strongly localized in the circumference direction; that is, ,A!x" is a wave function localized around x= ± #Ch# /2 at the bottom side of the cylinder, whereas ,B!x" is localized around the

FIG. 18. Energy dispersion relation of a !10,0" tube as a function of the dimensionless wave vector ==k.#T# /2# for several values of the dimensionless inverse magnetic length ;. !a" ;=0.0, !b" 1.0, !c" 2.0, and !d" 3.0. !e", !f", !g" The energy at k. =0 as a function of ;2 /NR 'NR is the highest common divisor of !2n+m ,n+2m"( for tubes !20,0", !20,20", and !9,9", respectively. Adapted from Saito, Dresselhaus, and Dresselhaus, 1994.

691Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

top side x=0. As a result, the boundary condition on the wave function becomes irrelevant and the resulting band structures, starting from an initially metallic or semicon- ducting nanotube, become identical !Ajiki and Ando, 1993". For a small +k around the K points, the low- energy properties are described by an effective Hamil- tonian, which can be determined by the two degenerate states ,A and ,B as

Heff = * 0 ! i.0+kI0 !1!2;2"

+ i.0+kI0 !1!2;2" 0

whose eigenvalues are Eq=0 ± = ±.0#+k# /I0!2;2", with a

group velocity given by v=.0 /1I0!2;2", while the density of states becomes 4!EF"/I0!2;2" /#.0/e;

2 /$4#;2!;

<1" !Ando and Seri, 1997". The DOS at the charge- neutrality point thus diverges exponentially with in- creasing magnetic field. This is shown in Fig. 19 for the !10,10" tube for several magnetic field strengths.

Given the diameter-dependent scaling property of the band structure, the larger the tube diameter, the smaller the required value of the magnetic field to fully develop such a Landau subband at the charge-neutrality point. This effect has also been investigated analytically using a supersymmetry framework !Lee and Novikov, 2003". The appearance of the so-called Hofstadter butterfly was further explored numerically for large diameter nanotubes !Nemec and Cuniberti, 2006". As already seen in the field-dependent band structures !Fig. 18", the whole DOS also progressively degrades as the Landau subbands start to emerge within the whole spectrum, al- though strong mixing between high-energy subbands re- mains !Fig. 19".

As soon as ;= #Ch# /2#!m>1 is satisfied, the electronic spectrum becomes fully dominated by Landau levels. One finds that for tubes with diameters of 1, 10, 20, and 40 nm, the condition ;=1 corresponds to magnetic field strengths of 2635, 26, 6.6, and 1.6 T, respectively.

In each case, !m?!e !or @c-e<1" has to be further satisfied for clear observation of Landau quantization, where !e is the mean free path, @c=eB /m is the cyclo- tron frequency, and -e is the scattering time !this condi- tion is easily met at such high magnetic fields in carbon nanotubes since !e can be as long as 1 "m". Some signa- ture of such Landau level formation was first reported by Kanda and co-workers !Kanda et al., 2002".

F. Curvature effects: Beyond the zone-folding model

In the preceding sections, a model for the electronic properties of SWNTs was based on the confinement of electrons around the tube circumference, a confinement shown to induce selection on allowed k! Bloch vector components. As a matter of fact, since the states se- lected in the band-folding scheme were those of the pla- nar graphene sheet, curvature effects are neglected. However, carbon nanotubes are not just stripes of graphene but small cylinders. Carbon atoms are placed on a cylindrical wall, a topology that induces several ef- fects different from those of a planar graphene sheet: !a" the C-C bonds perpendicular and parallel to the axis are slightly different, so that the a1 and a2 basis vectors now have different lengths; !b" these bond length changes, and the formation of an angle for the two pz orbitals located on bonds not strictly parallel to the axis, yield differences in the three hopping terms .0 between a car- bon atom and its three neighbors; and !c" the planar symmetry is broken so that the # and ' states can mix and form hybrid orbitals that exhibit partial sp2 and sp3

character. Such curvature effect is not taken into ac- count in the zone-folding model of graphene, where the # orbitals cannot mix with the ' states as they show different parity with respect to planar reflection. In the present section, the effect of finite curvature on the elec- tronic properties of single-wall nanotubes will be inves- tigated.

The effects labeled !a" and !b" modify the conditions that define the k point at which occupied and unoccu- pied bands do cross !a point we label kF" and shift this Fermi vector kF away from the Brillouin zone corners !K point" of the graphene sheet !Kane and Mele, 1997; Yang and Han, 2000". For armchair nanotubes, taking curvature into account shifts the Fermi wave vector along an allowed line of the graphene Brillouin zone. Consequently, for symmetry reasons, armchair tubes al- ways preserve their metallic character with finite curva- ture. However, for metallic nonarmchair nanotubes, kF moves away from the K point perpendicularly to the allowed k lines such that the allowed 1D subband !k ,q" no longer passes through kF, opening a very small band gap at EF !see Fig. 20".

In summary, when accounting for curvature effects, the only zero-band-gap tubes are the !n ,n" armchair nanotubes. The !n ,m" tubes with n!m=3l, where l is a nonzero integer, are tiny-gap semiconductors. Armchair tubes are sometimes labeled type-I metallic tubes, while the others are of type-II. All other nanotubes are

FIG. 19. Density of states of the !10,10" tube in a perpendicu- lar magnetic field for several field strengths. The field strengths are expressed in terms of the dimensionless parameter ; = #Ch# /2#!m, where !m=$1 /eB is the magnetic length.

692 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

intermediate-gap !a few tenths of an eV" semiconduc- tors. For the tiny-gap semiconducting nanotubes, the so- called secondary gap !due to the curvature" depends on the diameter and the chiral angle, and scales as 1/dt

2

!Kane and Mele, 1997". For the quasimetallic zigzag nanotubes !chiral angle=0", this secondary gap is given by

2Eg 2 =

3.0acc 2

4dt 2 !30"

and is so small that, for most practical purposes, all n !m=3l tubes can be considered as metallic at room tem- perature !see Fig. 20". Density-of-states measurements by scanning tunneling spectroscopy !Ouyang et al., 2001b" confirm the expected 1/dt

2 dependence for three zigzag nanotubes and show that armchair nanotubes re- main truly metallic. Consequently, the band-folding pic- ture, based on the tight-binding approach !Hamada et al., 1992; Mintmire et al., 1992; Saito et al., 1992", contin- ues to be valid for large diameter tubes.

We now discuss point !c". For small tubes, the curva- ture is so strong that some rehybridization among the ' and # states appears. In such a case, the zone-folding picture may fail completely and ab initio calculations should be performed to predict the electronic properties of small diameter nanotubes. As an example, the ab ini- tio band structure of the !6,0" tube is shown in Fig. 21. These first-principles pseudopotential local density func- tional !LDA" calculations !Blase, Benedict, Shirley, and Louie, 1994" indeed revealed that hybridization effects can occur in small radius nanotubes sufficiently strong to significantly alter their electronic structure. Strongly modified low-lying conduction band states are intro- duced into the band gap of insulating tubes because of

hybridization of the '* and #* states. As a result, the energy gaps of some small radius tubes are decreased by more than 50%. In the specific case of the !6,0" tube, which is predicted to be a semimetal in the band-folding scheme, a singly degenerate hybrid '*-#* state !see Fig. 21" is found to lie 0.83 eV !at (" below the doubly de- generate state that forms the top of the valence band in the zone-folding model. This band overlap makes the !6,0" tube a true metal within the LDA, with a density of states at the Fermi level equal to 0.07 state/eV atom. The '*-#* hybridization can be clearly observed by drawing the charge density associated with the states around the Fermi level. Such states are no longer anti- symmetric with respect to the tube wall, with a clear “charge spilling” out of the tube. For nanotubes with diameters greater than 1 nm, these rehybridization '-# effects are unimportant. Further, as discussed above, symmetry considerations suggest that armchair tubes are less affected by such rehybridization.

Ultrasmall radius single-wall carbon nanotubes !diam- eter of about 4 Å" have been produced by confining their synthesis inside inert AlPO4-5 zeolite channels !with inner diameter of about 7.3 Å" !Wang et al., 2000". The diameter of these tubes gives them many unusual properties such as superconductivity !Tang et al., 2001". Such a narrow distribution of diameters around 4 Å re- duces the potential carbon nanotube candidates to three: the !3,3", !4,2", and !5,0". The properties of these ultrasmall tubes have already been extensively investi- gated by ab initio simulations !Dubay et al., 2002; Liu and Chan, 2002; Machón et al., 2002; Cabria et al., 2003". In particular, it was shown that the !5,0" tube, expected to be semiconducting following the band-folding picture, is actually a metal with two bands !one doubly degener- ate" crossing the Fermi level !yielding two different kF".

FIG. 20. Magnitude of primary !Eg 1" and secondary !Eg

2" gaps in carbon nanotubes with radii less than 15 Å. The primary gap !2Eg

1" scales as 1/R !top panel". The secondary gap !2Eg 2

or cuvature-induced gap" scales as 1/R2. The dots at 2Eg 1

=2Eg 2=0 correspond to the armchair nanotubes which always

preserve their metallic character. Adapted from Kane and Mele, 1997.

FIG. 21. Ab initio electronic band structure and density of states of a !6,0" carbon nanotube, illustrating the strong hybrid- ization that occurs between # and ' states in a small-diameter tube. A new band '* appears and crosses the # states around the center of the Brillouin zone. The Fermi level is at zero energy. Adapted from Blase, Benedict, Shirley, and Louie, 1994.

693Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

This is a clear manifestation of curvature effects. We will come back to such small tubes when discussing the Peierls and superconducting instabilities in Sec. IV.F. The armchair !3,3" tube remains semimetallic, but with a #-#* band crossing at EF that is displaced off its ideal 2(X /3 position, confirming as described above that arm- chair tubes are much less sensitive to curvature effects.

G. Nanotube bundle and multiwall system

From the previous section, we can deduce that only a special achiral subset of these carbon structures !arm- chair nanotubes" exhibits a true metallic behavior. Such metallic character can be explained by the high symme- try of these !n ,n" tubes, namely, the n vertical planes and glide planes. Incorporating an armchair tube into a bundle, or inside another nanotube as in a multiwall sys- tem, could modify its intrinsic electronic properties as the symmetry is lowered.

Single-wall carbon nanotubes are grown by a laser- ablation, arc-discharge, or CVD method and always oc- cur in bundles of 10–100 nanotubes. These bundles usu- ally consist of nanotubes with different chirality and slightly different diameter. Even a “perfect” crystal made of identical tubes will alter the properties of the constituent CNTs through tube-tube interaction. Indeed, first-principles calculations reveal that broken symmetry of the !10,10" tube caused by interactions between tubes in a bundle induces a pseudogap of about 0.1 eV at the Fermi energy !Delaney et al., 1998". This pseudogap strongly modifies many of the fundamental electronic properties of the armchair tubes, with a specific signa- ture in the temperature dependence of the electrical conductivity and in the infrared absorption spectrum.

In the limit of an isolated !10,10" tube, the two bands crossing at EF belong to different irreducible represen- tations with respect to the tube symmetry planes, so that crossing is allowed. Upon breaking of this symmetry by tube-tube interaction in the hexagonal bundle symmetry, these bands can mix and start to repel at EF !Fig. 22". The presence and magnitude !which depends inversely on the nanotube radius" of this pseudogap have been observed experimentally using low-temperature scan-

ning tunneling spectroscopy !Ouyang et al., 2001b". In contrast, if !6,6" nanotubes are arranged in a hexagonal lattice which fully preserves the D6h symmetry of the hexagonal packing, the band gap due to these intertube interactions is not observed !Charlier et al., 1995". A small rotation of the !6,6" tubes in such an arrangement would break the D6h symmetry of the !6,6" bundle and would open up this expected gap at the Fermi energy !Reich, Thomsen, and Ordejón, 2002".

Another possibility to tailor the electronic properties of nanotubes can be observed in the multilayering effect. In fact, the weak interaction between the concentric shells in a multiwall nanotube may have important ef- fects on the electronic properties of the constituent iso- lated nanotubes !Lambin et al., 1994; Kwon and Tománek, 1998". Interwall coupling, which, as just men- tioned, opens a pseudogap in bundles of single-wall nanotubes !due to symmetry lowering", may periodically open and close four such pseudogaps near the Fermi energy in a metallic double-wall nanotube upon rotation of its inner shell with respect to the nanotube axis.

Figure 23 illustrates the intriguing interplay between geometry and electronic structure during the rotation of an inside !5,5" armchair nanotube in an outside !10,10" nanotube !both tubes sharing the same axis". The indi- vidual !5,5" and !10,10" tubes are both metallic and show the preferred graphitic interwall separation of 3.4 Å when nested. To determine the electronic properties of the double-wall nanotube, a tight-binding technique with parameters determined by ab initio calculations for simpler structures has been used !Lambin et al., 1994; Kwon and Tománek, 1998". Due to the relatively high symmetry of the coaxial system, consisting of a D10h !5,5" nanotube nested inside a D20h !10,10" nanotube, the de- pendence of the intertube interaction on the tube orien- tation shows a periodicity of 18°. In the absence of the intertube interaction, the band structure of each tube is characterized by two crossing linear bands near EF, one for left- and one for right-moving electrons. The band structure of a pair of decoupled !5,5" and !10,10" nano- tubes, a mere superposition of the individual band struc- tures, is shown in Fig. 23!a". Switching on the intertube interaction in the !5,5"@!10,10" double-wall tube re-

FIG. 22. Band crossing and band repulsion. !a" Schematic diagram of the crossing of the two linear bands for an isolated !n ,n" carbon nanotube. One band has #-bonding character and the other has #-antibonding !#*" character. EF is the Fermi energy and k is the wave vector. !b" Repulsion of the bands due to breaking of mirror symmetry. Adapted from Delaney et al., 1998.

694 Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

moves the near degeneracy of the bands near EF as well 'see Figs. 23!b" and 23!c"(. In the most stable orienta- tion, the double-wall system is still characterized by the D10h symmetry of the inner tube. The four bands cross, with a very small change in the slope 'Fig. 23!b"(. While the same argument also applies to the least-stable con- figuration, a markedly different behavior is obtained at any other tube orientation that lowers the symmetry, giving rise to four band crossings 'Fig. 23!c"(. This trans- lates into four pseudogaps in the density of states near EF.

At the Fermi level, the density of states of double-wall nanotubes is thus affected by the mutual orientation of the two constituent nanotubes, since the positions of the four pseudogaps depend significantly on it. The opening and closing of pseudogaps during the libration motion of the double-wall tube is a unique property that cannot be observed in single-wall nanotube ropes !Kwon and Tománek, 1998".

Finally, self-consistent charge-density and potential profiles for double-wall nanotubes, considering various chiralities, have been determined !Miyamoto et al., 2001" and demonstrate that the inner tube modifies the charge density associated with states near EF, even outside the outer tube. A significant amount of charge, originating mainly from # electrons, is transferred into an interwall state, related to the interlayer state in graphite. In the limit of small tubes, the significant evolution of the CNT work function with respect to diameter shows as well that charge transfer may occur from one tube to another.

H. Structural defects in carbon nanotubes

In the previous sections, curvature effects and inter- tube and intershell interactions have been shown to sig- nificantly modify the electronic properties of carbon nanotubes from those obtained by a simple band folding of the graphene band structure. However, until now, each constituent nanotube was assumed to be perfect. In reality, the intrinsic honeycomb network of CNTs is probably not as perfect as usually assumed. Defects like pentagons, heptagons, vacancies, adatoms, or substitu-

tional impurities have been proposed theoretically and recently observed experimentally !Hashimoto et al., 2004; Fan et al., 2005". These defects are found to modify, at least locally, the electronic properties of the host nanotubes. Consequently, the introduction of de- fects in the carbon network is an interesting way to tai- lor its intrinsic properties, enabling new potential nano- devices and fostering innovative applications in nano- electronics !Gómez-Navarro et al., 2005". The cases of chemical doping and functionalization will be explored in Sec. IV.C.4 where their effect on conductance will be analyzed.

1. Finite length and capping topologies

We have dealt so far with the properties of infinitely long nanotubes. In reality, nanotubes have a finite length !up to a few microns", a property which has two main consequences: !a" the confinement of the electronic states along the tube length; and !b" the disruption of the atomic network at the two ends, also labeled tips or apexes, with specific reconstructions and local electronic properties.

A conducting nanotube cut to a finite length should display standing waves characteristic of a one- dimensional particle-in-a-box model. Indeed, when elec- trons are confined in a box, quantum mechanics tells us that electrons can have only discrete values of kinetic energy. The energy spacing of the eigenvalues depends directly on the dimensions of the box: 2E=h2 /2mL2, with L the length of the box. If this energy spacing is much higher than the thermal energy !2E<kBT", there are only completely occupied and completely empty lev- els and the system is an insulator. Further, the eigen- states are standing waves of the form sin!kz", with k =2#m /L and m an integer !the variable z is along the nanotube axis".

These standing waves have been studied theoretically by Rubio et al. !1999", and the highest occupied molecu- lar orbital !HOMO", lowest unoccupied molecular or- bital !LUMO", and “tip states” associated with a typical finite-length tube are illustrated in Fig. 24. Such station- ary states have also been observed experimentally by

FIG. 23. Band structures of the same double-wall tube for different relative orientations. Near-degenerate bands with no gap characterize the !5,5"@!10,10" double-wall nanotube without intertube interaction !a". In the presence of intertube interaction, depending on the mutual tube orientation, the !5,5"@!10,10" system may show a zero gap !b" in the most symmetric !point group symmetry D10h" or four pseudogaps !c" in a less symmetric and stable configuration !point group symmetry C5". Adapted from Kwon and Tománek, 1998.

695Charlier, Blase, and Roche: Electronic and transport properties of nanotubes

Rev. Mod. Phys., Vol. 79, No. 2, April–June 2007

means of STS !Venema et al., 1999; Lemay et al., 2001" which essentially sees the square of the wave functions close to the Fermi level 'dI!V ,x" /dV/#,F!x"#2(. The STS scans display several maxima repeated with a peri- odicity :F60.74 nm. Such an observation requires a higher energy resolution than the eigenstate separation !2E" and an electron coherence length larger than the tube length, which was satisfied for Ltube/30 nm and T=4 K.

We now turn to the properties of tube tips or apexes. Due to the finite length, interesting structural features occur near t